Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

574 views

Published on

No Downloads

Total views

574

On SlideShare

0

From Embeds

0

Number of Embeds

2

Shares

0

Downloads

0

Comments

0

Likes

1

No embeds

No notes for slide

- 1. Multipole Expansion Method in Micromechanics of Composites Volodymyr I. Kushch Introduction In scientiﬁc literature, the Multipole Expansion Method is associated with a group of techniques and algorithms designed to study behavior of large scale collections of interacting objects of various nature, from atoms and molecules up to stars and galaxies. Analytical in nature, this method provides a theoretical basis of very efﬁ- cient (e.g., [18]) computer codes and found numerous applications in cosmology, physics, chemistry, engineering, statistics, etc. This list includes also mechanics of heterogeneous solids and ﬂuid suspensions, where a certain progress is observed in development of the multipole expansion based theories and applications. The author’s opinion is, however, that importance of this method for the micro- mechanics of composites is underestimated and its potential in the area is still not fully discovered. The contemporary studies on composites are still often based on the single inclusion model even if this is inappropriate in the problem under study. As known, the single inclusion-based theories provide O(c) estimate of effective properties, c being the volume content of inclusions, so their application is justiﬁed to the composites with low c only. In order to get the next, O(c2) virial expansion term of the effective property, the pair interaction effect must be taken into account by means of the two-inclusion model (e.g., [26]). Further accuracy improvement requires the model with several interacting inclusions to be considered. The multi- pole expansion is an efﬁcient tool for studying, from the multiple inclusion models, the effects caused by micro structure on the local ﬁelds and effective properties being the central problem of the science of composites. It should be mentioned that some diversity exists in literature in using the words “multipole” and “multipole expansion”. The idea of multipoles is traced back to V. I. Kushch Institute for Superhard Materials, Kiev, Ukraine e-mail: vkushch@bigmir.net M. Kachanov and I. Sevostianov (eds.), Effective Properties of Heterogeneous Materials, 97 Solid Mechanics and Its Applications 193, DOI: 10.1007/978-94-007-5715-8_2, © Springer Science+Business Media Dordrecht 2013
- 2. 98 V. I. Kushch Maxwell [57] who deﬁned them as the complex point charges and studied the relationship between the potential ﬁelds of multipoles and spherical harmonics. To avoid confusing, the notions “multipole” (point source), “multipole ﬁeld” (poten- tial) and “multipole moment” (strength) should be clearly distinguished. Among sev- eral available in literature deﬁnitions, the most general one, probably, is [25]: “...A multipole expansion is a series expansion of the effect produced by a given system in terms of an expansion parameter which becomes small as the distance away from the system increases”. The basis functions and the expansion coefﬁcients are referred as the potential ﬁelds and moments (strengths) of multipoles, respectively. What is important, this deﬁnition imposes no restrictions on the basis functions and, in what follows, we accept it. By tradition, we call the method exposed in this Chapter the Multipole Expan- sion Method (MEM) despite the fact that multipole expansion is only a part of solution procedure. The basic idea of the method consists in reducing the boundary value problem stated on the piece-homogeneous domain to the ordinary system of linear algebraic equations. In so doing, a considerable analytical effort involving the mathematical physics and theory of special functions is required. This effort is quite rewarding, in view of the obtained this way remarkably simple and efﬁcient computational algorithms. MEM is essentially the series method, where the partial solutions of differential equation obtained by separation of variables in an appropriate coordinate system constitute a countable set of basis functions. The speciﬁc curvilinear coordinate system is dictated by the inclusion shape and introduced in a way that the matrix- inclusion interface coincides with the coordinate surface. An important for our study feature of the basis functions is that at this coordinate surface they form a full and orthogonal set of surface harmonics and thus provide an efﬁcient way of fulﬁlling the interface boundary conditions. In this Chapter, we review the work done for the scalar (conductivity) and vec- torial (linear elasticity) problems. Two matrix type composites under study are (a) particulate composites with spherical and spheroidal inclusions and (b) unidirec- tional ﬁbrous composite materials with circular and elliptic (in cross-section) ﬁbers. The isotropic as well as anisotropic properties of constituents are considered. The review is structured as follows. The homogenization problem, in particular, the rational way of introducing the macro parameters and effective properties of composite is brieﬂy discussed in Sect.1. The general formulas for the macroscopic ﬂux vector and stress tensor are derived in terms of corresponding average gradient ﬁelds and dipole moments (stresslets) of the disturbance ﬁelds, i.e., in the form most appropriate for the multipole expansion approach.
- 3. Multipole Expansion Method in Micromechanics of Composites 99 In Sect.2, we consider the Multipole Expansion Method in application to con- ductivity of composite with spherical inclusions as the most widely used and traditionally associated with multipoles geometry. This problem is well explored and we revisit it with aim to demonstrate the basic technique of the method and discuss the principal moments. In the subsequent Sections, the Multipole Expansion Method is applied to the elasticity problem as well as expanded on the composites with more complicated geometry of inclusions and properties of constituents. All the Sections are structured uniformly, in accordance with the MEM solution ﬂow. We begin with the problem for a single inclusion, immersed in non-uniform far ﬁeld. These results, on the one hand, provide a necessary background for the subsequent study. On the other hand, they can be viewed as the generalized Eshelby’s model expanded on the case of non-uniform far load—but still readily implanted in that or another self-consistent scheme. Next, the Finite Cluster Model (FCM) is considered. To obtain an accurate solu- tion of the multiple inclusion problem, the above solution for a single inclusion is combined with the superposition principle and the re-expansion formulas for a given geometry of inclusion. These results constitute the intermediate, second step of the method and will be further developed in order to obtain the full-featured model of composite. At the same time, this model can be viewed as the gen- eralized Maxwell’s model, where the particle-particle interactions are taken into account. Then, the Representative Unit Cell (RUC) model of composite is studied. Here, the periodic solutions and corresponding lattice sums are introduced. A complete solution of the model provides a detailed analysis of the local ﬁelds, their ana- lytical integration gives the exact, only dipole moments containing expressions of the effective conductivity and elasticity tensors.This model can be viewed as the generalized Rayleigh’s model expanded on the general type geometry (both regular and random) of composite, with an adequate account for the interaction effects. 1 Homogenization Problem The homogenization problem is in the focus of the composite mechanics for the last 50years. The various aspects of this problem including (a) structure levels, (c) representative volume element (RVE) size and shape, (b) way of introducing the macro parameters and effective properties of composite, etc., were widely discussed in several books and thousands of papers. Our aim is more limited and speciﬁc: here, we will discuss how the multipole expansion solutions apply to the homogenization problem.
- 4. 100 V. I. Kushch 1.1 Conductivity 1.1.1 Deﬁnition of Macroscopic Quantities: Volume Versus Surface Averaging The macroscopic, or effective, conductivity tensor ∗ = λ∗ i j is deﬁned by the Fourier law: q = − ∗ · ∇T . (1.1) In (1.1), ∇T and q are the macroscopic temperature gradient and heat ﬂux vector, respectively. Their introduction is not as self-obvious and the researchers are not unanimous in this matter. In most publications, ∇T and q are taken as the volume- averaged values of corresponding local ﬁelds: ∇T = 1 V V ∇T dV ; q = 1 V V qdV ; (1.2) where V is a volume of the representative volume element (RVE) of composite solid. For the matrix type composite we consider, V = N q=0 Vq, Vq being the volume of qth inclusion and V0 being the matrix volume inside RVE. An alternate, surface averaging-based deﬁnition of the macroscopic conductivity parameters is [90]: ∇T = 1 V S0 T ndS, q = 1 V S0 (q · n) rdS. (1.3) It is instructive to compare these two deﬁnitions. We employ the gradient theorem [64] to write 1 V V ∇T dV = 1 V S0 T (0) ndS + 1 V N q=1 Sq T (q) − T (0) ndS, (1.4) where Sq is the surface of Vq, S0 is the outer surface of RVE and n is the unit normal vector. As seen from (1.4), the compared formulas coincide only if temperature is continuous T (0) = T (q) at the interface. Noteworthy, (1.3) holds true for com- posites with imperfect interfaces whereas (1.2) obviously not. On order to compare two deﬁnitions of q , we employ the identity q = ∇ · q ⊗ r and the divergence theorem [64] to get 1 V V qdV = 1 V S0 q(0) · n rdS + 1 V N q=1 Sq q(q) · n − q(0) · n rdS.
- 5. Multipole Expansion Method in Micromechanics of Composites 101 Again, two deﬁnitions coincide only if the normal ﬂux qn = q · n is continuous across the interface—and again Eq.(1.3) holds true for composites with imperfect interfaces. Thus, (1.2) is valid only for the composites with perfect thermal contact between the constituents. The deﬁnition (1.3) is advantageous at least in the following aspects: • It involves only the observable quantities—temperature and ﬂux—at the surface of composite specimen. In essence, we consider RVE as a “black box” whose interior structure may affect numerical values of the macro parameters—but not the way they were introduced. • This deﬁnition is valid for composites with arbitrary interior microstructure and arbitrary (not necessarily perfect) interface bonding degree as well as for porous and cracked solids. • Numerical simulation becomes quite similar to (and reproducible in) the exper- imental tests where we apply the temperature drop (voltage, etc.) to the surface of specimen and measure the heat ﬂux (current, etc.) passing the surface. Macro- scopic conductivity of composite is then found as the output-to-input ratio. In so doing, we have no need to study interior microstructure of composite and/or perform volume averaging of the local ﬁelds. 1.1.2 Formula for Macroscopic Flux Now, we derive the formula, particularly useful for the effective conductivity study by the Multipole Expansion Method. We start with the generalized Green’s theorem V (uLv − vLu)dV = S u ∂v ∂M − v ∂u ∂M dS, (1.5) where Lu = m i, j=1 λi j ∂2u ∂xi ∂xj , ∂u ∂M = m i, j=1 λi j n j ∂u ∂xi . (1.6) In our context, m = 2 or 3. Physical meaning of the differential operators (1.6) is clear from the formulas Lu = ∇ · ( · ∇u) = −∇ · q(u); ∂u ∂M = ( · ∇u) · n = −qn(u). (1.7) WeapplyEqs.(1.5) and(1.7) tothematrixpart (V0) of RVE: withnoloss ingenerality, we assume the outer boundary of RVE S0 entirely belonging to the matrix. In new notations,
- 6. 102 V. I. Kushch V0 T (0) ∇ · q T − T ∇ · q T (0) dV = N q=0 Sq T (0) qn T − T qn T (0) dS, (1.8) where T (0) is an actual temperature ﬁeld in matrix phase of composite and T is a trail temperature ﬁeld obeying, as well as T (0), the energy conservation law ∇ ·q (T ) = 0 in every point of V0. Therefore, the volume integral in the left hand side of (1.8) is identically zero. In the right hand side of (1.8), we take T = xk and multiply by the Cartesian unit vector ik to get N q=0 Sq T (0) 0 · n + qn T (0) r ds = 0, where r = xkik is the radius-vector and n = nkik is the unit normal vector to the surface Sq. In view of qn T (0) = q T (0) · n and (1.3), we come to the formula q = − 0 · ∇T + 1 V N q=1 Sq T (0) qn r − qn(T (0) )r ds, (1.9) where we denote qn(r) = qn(xk)ik. This formula is remarkable in several aspects. • First, and most important, this equation together with (1.1) provide evaluation of the effective conductivity tensor of composite solid. Using RUC as the represen- tative volume enables further simpliﬁcation of Eq.(1.9). • In derivation, no constraints were imposed on the shape of inclusions and inter- face conditions. Therefore, (1.9) is valid for the composite with anisotropic con- stituents and arbitrary matrix-to-inclusion interface shape, structure and bonding type. • Integrals in (1.9) involve only the matrix phase temperature ﬁeld, T (0). Moreover, these integrals are identically zero for all but dipole term in the T (0) multipole expansion in a vicinity of each inclusion and, in fact, represent contribution of these inclusions to the overall conductivity tensor. • In the Multipole Expansion Method, where temperature in the matrix is initially taken in the form of multipole expansion, an analytical integration in (1.9) is straightforward and yields the exact, ﬁnite form expressions for the effective properties.
- 7. Multipole Expansion Method in Micromechanics of Composites 103 1.2 Elasticity The fourth rank effective elastic stiffness tensor C∗ = C∗ i jkl is deﬁned by σ = C∗ : ε , (1.10) where the macroscopic strain ε and stress σ tensors are conventionally deﬁned as volume-averaged quantities: ε = 1 V V εdV ; σ = 1 V V σdV. (1.11) This deﬁnition is valid for the composites with perfect mechanical bonding—and fails completely for the composites with imperfect interfaces. Also, this deﬁnition is “conditionally” correct for the porous and cracked solids. Analogous to (1.3) surface averaging-based deﬁnition of the macroscopic strain and stress tensors [4] ε = 1 2V S0 (n ⊗ u + u ⊗ n) dS; σ = 1 V S0 r ⊗ (σ · n) dS; (1.12) resolves the problem. In the case of perfect interfaces, this deﬁnition agrees with the conventional one, (1.11). This result is known in elastostatics as the mean strain the- orem (e.g., [20]). Also, it follows from the mean stress theorem [20] that the volume averaged σ in (1.11) is consistent with (1.12) in the case of perfect mechanical contact between the matrix and inclusions. What is important for us, (1.12) holds true for the composites with imperfect interfaces (e.g., [11]). 1.2.1 Formula for Macroscopic Stress The Betti’s reciprocal theorem [20] written for the matrix domain V0 of RVE states that the equality N q=0 Sq Tn(u(0) ) · u − Tn(u ) · u(0) dS = 0 is valid for any displacement vector u obeying the equilibrium equation ∇ · (C : ∇u) = 0. Following [44], we take it in the form ui j = ii xj . The dot product Tn(u(0)) · ui j = σ (0) il nlxj and, by deﬁnition (1.12), S0 Tn(u(0) ) · ui j dS = V σi j .
- 8. 104 V. I. Kushch On the other hand, Tn(ui j ) · u(0) = σkl(ui j )nlu− k = C (0) i jklnlu− k ; comparison with (1.12) gives us 1 V S0 Tn(ui j ) · u(0) dS = C (0) i jkl εkl . Thus, we come out with the formula σi j = C (0) i jkl εkl + 1 V N q=1 Sq Tn(u(0) ) · ui j − Tn(ui j ) · u(0) dS (1.13) consistent with [74]. The Eq.(1.13) is the counterpart of (1.9) in the elasticity theory and everything said above with regard to (1.9) holds true for (1.13). • This formula is valid for the composite with arbitrary (a) shape of disperse phase, (b) anisotropy of elastic properties of constituents and (c) interface bonding type. • Together with (1.10), (1.13) enables evaluation of the effective stiffness tensor of composite provided the local displacement ﬁeld u(0) is known/found in some way. • An yet another remarkable property of this formula consists in that the integral it involves (stresslet, in [74] terminology) is non-zero only for the dipole term in the vector multipole expansion of u(0). 2 Composite with Spherical Inclusions: Conductivity Problem The multipoles are usually associated with the spherical geometry, and the most work in the multipoles theory have been done for this case. In particular, the conductiv- ity problem for a composite with spherical inclusions has received much attention starting from the pioneering works of Maxwell [57] and Rayleigh [73]. Now, this problem has been thoroughly studied and we revisit it to illustrate the basic technique of the method. To be speciﬁc, we consider thermal conductivity of composite. These results apply also to the mathematically equivalent physical phenomena (electric conductivity, diffusion, magnetic permeability, etc.).
- 9. Multipole Expansion Method in Micromechanics of Composites 105 2.1 Background Theory 2.1.1 Spherical Harmonics The spherical coordinates (r, θ, ϕ) relate the Cartesian coordinates (x1, x2, x3) by x1 + ix2 = r sin θ exp(iϕ), x3 = r cos θ (r ≥ 0, 0 ≤ θ ≤ π, 0 ≤ ϕ < 2π). (2.1) Separation of variables in Laplace equation ΔT (r) = 0 (2.2) in spherical coordinates gives us a set of partial (“normal”, in Hobson’s [23] termi- nology) solutions of the form rt Ps t (cos θ) exp(isϕ) (−∞ < t < ∞, −t ≤ s ≤ t) (2.3) referred [57] as scalar solid spherical harmonics of degree t and order s. Here, Ps t are the associate Legendre’s functions of ﬁrst kind [23]. With regard to the asymptotic behavior, the whole set (2.3) is divided into two subsets: regular (inﬁnitely growing with r → ∞) and singular (tending to zero with r → ∞) functions. We denote them separately as ys t (r) = rt (t + s)! χs t (θ, ϕ); Ys t (r) = (t − s)! rt+1 χs t (θ, ϕ) (t ≥ 0, |s| ≤ t), (2.4) respectively. In (2.4), χs t are the scalar surface spherical harmonics χs t (θ, ϕ) = Ps t (cos θ) exp(isϕ). (2.5) They possess the orthogonality property 1 S S χs t χl k dS = αtsδtkδsl, αts = 1 2t + 1 (t + s)! (t − s)! , (2.6) where integral is taken over the spherical surface S; over bar means complex con- jugate and δi j is the Kronecker’s delta. Adopted in (2.4) normalization is aimed to simplify the algebra [29, 71]: so, we have y−s t (r) = (−1)sys t (r), Y−s t (r) = (−1)sYs t (r). (2.7) We mention also the differentiation rule [23]:
- 10. 106 V. I. Kushch D1ys t = ys−1 t−1 , D2ys t = −ys+1 t−1 , D3ys t = ys t−1; D1Ys t = Ys−1 t+1 , D2Ys t = −Ys+1 t+1 , D3Ys t = −Ys t+1; (2.8) or, in the compact form, (D2)s (D3)t−s 1 r = (−1)t Ys t (r) (2.9) where Di are the differential operators D1 = ∂ ∂x1 − i ∂ ∂x2 , D2 = D1 = ∂ ∂x1 + i ∂ ∂x2 , D3 = ∂ ∂x3 . (2.10) These operators can be viewed as the directional derivatives along the complex Cartesian unit vectors ei deﬁned as e1 = (i1 + ii1)/2, e2 = e1, e3 = i3. (2.11) 2.1.2 Spherical Harmonics Versus Multipole Potentials Maxwell [57] has discovered the relationship between the solid spherical harmonics (2.7) and the potential ﬁelds of multipoles. So, the potential surrounding a point charge (being a singular point of zeroth order, or monopole) is 1/r = Y0 0 (r). The ﬁrst order singular point, or dipole, is obtained by pushing two monopoles of equal strength—but with opposite signs—toward each other. The potential of the dipole to be given (up to rescaling) by the directional derivative ∇u1 (1/r), where u1 is the direction along which the two monopoles approach one another. Similarly, pushing together two dipoles with opposite signs gives (up to rescaling) a quadrupole with potential ∇u1 ∇u2 (1/r), where u2 s the direction along which the dipoles approach, and so on. In general, the multipole of order t is constructed with aid of 2t point charges and has the potential proportional to ∇u1 ∇u2 . . . ∇ut (1/r). The latter can be expanded into a weighted sum of 2t + 1 spherical harmonics of order t, i.e., Ys t (r), −t ≤ s ≤ t. And, vise versa, Ys t (r) can be written as ∇u1 ∇u2 . . . ∇ut (1/r) provided the directions ui are taken in accordance with the formula (2.9). This is why the series expansion in terms of solid spherical harmonics (2.7) is often referred as the multipole expansion. 2.2 General Solution for a Single Inclusion Let consider the regular, non-uniform temperature far ﬁeld Tf ar in unbounded solid (matrix) of conductivity λ0. We insert a spherical inclusion of radius R and
- 11. Multipole Expansion Method in Micromechanics of Composites 107 conductivity λ1 inclusion assuming that its presence does not alter the incident ﬁeld. The inclusion causes local disturbance Tdis of temperature ﬁeld vanishing at inﬁnity and depending, besides Tf ar , on the shape and size of inclusion, conductivities of the matrix and inclusion materials and the matrix-inclusion bonding type. The tem- perature ﬁeld T (T = T (0) in the matrix, T = T (1) in the inclusion) satisﬁes (2.2). At the interface S (r = R), the perfect thermal contact is supposed: [[T ]] = 0; [[qr ]] = 0; (2.12) where [[ f ]] = ( f (0) − f (1))|r=R is a jump of quantity f through the interface S and qn = −λ∇T · n is the normal heat ﬂux. Our aim is to determine the temperature in and outside the inclusion. 2.2.1 Multipole Expansion Solution The temperature ﬁeld in the inclusion T (1) is ﬁnite and hence its series expansion contains the regular solutions ys t (r) (2.4) only: T (1) (r) = ∞ t=0 t s=−t dtsys t (r) (2.13) where dts are the unknown coefﬁcients (complex, in general). Temperature is a real quantity, so (2.7) leads to analogous relation between the series expansion coefﬁ- cients: dt,−s = (−1)sdts. In accordance with physics of the problem, temperature T (0) in the matrix domain is written as T (0) = Tf ar + Tdis, where Tdis(r) → 0 with r → ∞. It means that Tdis series expansion contains the singular solutions Ys t only. So, we have T (0) (r) = Tf ar (r) + ∞ t=1 t s=−t AtsYs t (r), (2.14) where Ats are the unknown coefﬁcients. Again, At,−s = (−1)s Ats. The second, series term in (2.14) is the multipole expansion of the disturbance ﬁeld Tdis. 2.2.2 Far Field Expansion We consider Tf ar as the governing parameter. It can be prescribed either analytically or in tabular form (e.g., obtained from numerical analysis). In fact, it sufﬁces to know Tf ar values in the integration points at the interface S deﬁned by r = R. Due to regularity of Tf ar in a vicinity of inclusion, its series expansion is analogous to (2.13), with the another set of coefﬁcients cts. In view of (2.6), they are equal to
- 12. 108 V. I. Kushch cts = (t + s)! 4πR2αts S Tf ar χs t dS. (2.15) For a given Tf ar , we can consider cts as the known values. Integration in (2.15) can be done either analytically or numerically: in the latter case, the appropriate scheme [42] comprises uniform distribution of integration points in azimuthal direction ϕ with Gauss-Legendre formula [1] for integration with respect to θ. 2.2.3 Resolving Equations The last step consists is substituting T (0) (2.14) and T (1) (2.13) into the bonding conditions (2.12). From the ﬁrst, temperature continuity condition we get for r = R ∞ t=0 t s=−t cts Rt (t + s)! χs t (θ, ϕ) + ∞ t=1 t s=−t Ats (t − s)! Rt+1 χs t (θ, ϕ) (2.16) = ∞ t=0 t s=−t dts Rt (t + s)! χs t (θ, ϕ). From here, for t = 0 (χ0 0 ≡ 1) we get immediately d00 = c00. For t = 0, in view of χs t orthogonality property (2.6), we come to a set of linear algebraic equations (t − s)! (t + s)! R2t+1 Ats + cts = dts. (2.17) The second, normal ﬂux continuity condition gives us also − (t + 1) t (t − s)! (t + s)! R2t+1 Ats + cts = ωdts, (2.18) where ω = λ1/λ0. By eliminating dts from (2.17) to (2.18), we get the coefﬁ- cients Ats: (ω + 1 + 1/t) (ω − 1) (t − s)! (t + s)! R2t+1 Ats = −cts; (2.19) then, the dts coefﬁcients can be found from (2.17). The obtained general solution is exact and, in the case of polynomial far ﬁeld, ﬁnite one. 2.3 Finite Cluster Model (FCM) Now, we consider an unbounded solid containing a ﬁnite array of N spherical inclu- sions of radius Rq and conductivity λq centered in the points Oq. In the (arbitrarily
- 13. Multipole Expansion Method in Micromechanics of Composites 109 introduced) global Cartesian coordinate system Ox1x2x3, position of qth inclusion is deﬁned by the vector Rq = X1qex1 + X2qex2 + X3qex3, q = 1, 2, . . . , N. Their non-overlapping condition is Rpq > Rp + Rq, where the vector Rpq = Rq − Rp gives relative position of pth and qth inclusions. We introduce the local, inclusion- associated coordinate systems Ox1qx2qx3q with origins in Oq. The local variables rp = r − Rp of different coordinate systems relate each other by rq = rp − Rpq. 2.3.1 Superposition Principle A new feature of this problem consists in the following. Now, a given inclusion undergoes a joint action of incident far ﬁeld and the disturbance ﬁelds caused by all other inclusions. In turn, this inclusion affects the ﬁeld around other inclusions. This means that the problem must be solved for all the inclusions simultaneously. For this purpose, we apply the superposition principle widely used for tailoring the solution of linear problem in the multiple-connected domain. This principle [81] states that a general solution for the multiple-connected domain can be written as a superposition sum of general solutions for the single-connected domains whose intersection gives the considered multiple-connected domain. The derived above general solution for a single-connected domain allows to write a formal solution of the multiple inclusion problem. Moreover, the above exposed integration based expansion procedure (2.15) provides a complete solution of the problem. An alternate way consists in using the re-expansion formulas (referred also as the addition theorems) for the partial solutions. This way does not involve integration and appears more computationally efﬁcient. The re-expansion formulas is the second component added to the solution procedure at this stage. 2.3.2 Re-Expansion Formulas In notations (2.4), the re-expansion formulas for the scalar solid harmonics take the simplest possible form. Three kinds of re-expansion formulas are: singular-to-regular (S2R) Ys t (r + R) = ∞ k=0 k l=−k (−1)k+l Ys−l t+k (R)yl k(r), r < R ; (2.20) regular-to-regular (R2R) ys t (r + R) = t k=0 k l=−k ys−l t−k(R)yl k(r); (2.21)
- 14. 110 V. I. Kushch and singular-to-singular (S2S) Ys t (r + R) = ∞ k=t k l=−k (−1)t+k+s+l ys−l k−t (R)Yl k(r), r > R . (2.22) The formula (2.21) is ﬁnite and hence exact and valid for any r and R. In [77], (2.21) and (2.22) are regarded as translation of regular and singular solid harmonics, respectively. In [19], they are called translation of local and multipole expansions whereas (2.20) is referred as conversion of a multipole expansion into a local one. The formulas (2.20)–(2.22) can be derived in several ways, one of them based on using the formula (2.15). Noteworthy, these formulas constitute a theoretical background of the Fast Multipole Method [19]. 2.3.3 Multipole Expansion Theorem To illustrate the introduced concepts and formulas, we consider a standard problem of the multipoles theory. Let N monopoles of strength qp are located at the points Rp. We need to ﬁnd the multipole expansion of the total potential ﬁeld in the point r where r > Rs and Rs = maxp Rp . In other words, we are looking for the multipole expansion outside the sphere of radius Rs containing all the point sources. Since the monopoles possess the ﬁxed strength and do not interact, the total potential is equal to T (r) = N p=1 qp r − Rp (2.23) being a trivial case of the superposition sum. Next, by applying the formula (2.22) for t = s = 0, namely, 1 r − Rp = Y0 0 (r − Rp) = ∞ t=0 t s=−t ys t (Rp)Ys t (r), (2.24) valid at r > Rs for all p, one ﬁnds easily T (r) = ∞ t=0 t s=−t AtsYs t (r), Ats = N p=1 qpys t (Rp). (2.25) For the truncated (t ≤ tmax) series (2.25), the following error estimate exists: T (r) − tmax t=0 t s=−t AtsYs t (r) ≤ A (Rs/r)tmax+1 r − Rs , A = N p=1 |qp|. (2.26)
- 15. Multipole Expansion Method in Micromechanics of Composites 111 These results constitute the multipole expansion theorem [19]. The more involved problem for the multiple ﬁnite-size, interacting inclusions is considered below. 2.4 FCM Boundary Value Problem Let temperature ﬁeld T = T (0) in a matrix, T = T (p) in the pth inclusion of radius Rp and conductivity λ = λp. On the interfaces rp = Rp, perfect thermal contact (2.12) is supposed. Here, rp, θp, ϕp are the local spherical coordinates with the origin Op in the center of the pth inclusion. 2.4.1 Direct (Superposition) Sum In accordance with the superposition principle, T (0) (r) = Tf ar (r) + N p=1 T (p) dis (rp) (2.27) where Tf ar = G · r = Gi xi is the linear far ﬁeld, and T (p) dis (rp) = ∞ t=1 t s=−t A (p) ts Ys t (rp) (2.28) is a disturbance ﬁeld caused by pth inclusion centered in Op: T (p) dis (rp) → 0 with rp → ∞. 2.4.2 Local Series Expansion In a vicinity of Oq, the following expansions are valid: Tf ar (rq) = ∞ t=0 t s=−t c (q) ts ys t (rq), (2.29) where c (q) 00 = G · Rq, c (q) 10 = G3, c (q) 11 = G1 − iG2, c (q) 1,−1 = −c (q) 11 and c (q) ts = 0 otherwise. In (2.27), T (q) dis is already written in qth basis. For p = q, we apply the re-expansion formula (2.20) to get
- 16. 112 V. I. Kushch T (p) dis (rq) = ∞ t=0 t s=−t a (q) ts ys t (rq), a (q) ts = (−1)t+s N p=q ∞ k=1 k l=−k A (p) kl Yl−s k+t (Rpq). (2.30) By putting all the parts together, we get T (0) (rq) = ∞ t=1 t s=−t A (q) ts Ys t (rq) + ∞ t=0 t s=−t a (q) ts + c (q) ts ys t (rq) (2.31) and the problem is reduced to the considered above single inclusion study. 2.4.3 Inﬁnite Linear System By substituting T (0) (2.31) and T (q) (2.13) written in local coordinates into (2.12), we come to the set of equations with unknowns A (q) ts , quite analogous to (2.17). Namely, (ωq + 1 + 1/t) (ωq − 1) (t − s)! (t + s)! Rq 2t+1 A (q) ts + a (q) ts = −c (q) ts (ωq = λq/λ0); (2.32) or, in an explicit form, (ωq + 1 + 1/t) (ωq − 1) (t − s)! (t + s)! Rq 2t+1 A (q) ts (2.33) + (−1)t+s N p=q ∞ k=1 k l=−k A (p) kl Yl−s k+t (Rpq) = −c (q) ts . A total number of unknowns in (2.33) can be reduced by a factor two by taking account of A (p) k,−l = (−1) l A (p) kl . The theoretical solution (2.33) we found is formally exact—but, in contrast to (2.17), leads to the inﬁnite system of linear algebraic equations. The latter can be solved, with any desirable accuracy, by the truncation method provided a sufﬁcient number of harmonics (with t ≤ tmax) is retained in solution [17, 27]. Hence, the numerical solution of the truncated linear system can be regarded as an asymp- totically exact, because any accuracy can be achieved by the appropriate choice of tmax. The smaller distance between the inhomogeneities is, the higher harmon- ics must be retained in the numerical solution to ensure the same accuracy of computations.
- 17. Multipole Expansion Method in Micromechanics of Composites 113 2.4.4 Modiﬁed Maxwell’s Method for Effective Conductivity Since we have A (q) ts found from (2.33), one can evaluate the temperature ﬁeld in any point in and around the inclusions. Moreover, this model allows to evalu- ate an effective conductivity of composite with geometry represented by FCM. In fact, it was Maxwell [57] who ﬁrst suggested this model and derived his famous formula by equating “the potential at a great distance from the sphere” (in fact, total dipole moment) of an array of inclusions to that of the equivalent inclusion with unknown effective conductivity. In so doing, Maxwell neglected interaction between the inclusions—but wrote “...when the distance between the spheres is not great compared with their radii..., then other terms enter into the result which we shall not now consider.” Our solution contains all the terms and hence one can expect better accuracy of the Maxwell’s formula. In our notations, it takes the form λef f λ0 = 1 − 2c A10 1 + c A10 , (2.34) where λef f is the effective conductivity of composite with volume content c of spherical inclusions, the mean dipole moment A10 = 1 N N p=1 A (p) 10 and A (p) 10 are calculated from (2.33) for G3 = 1. Recently, this approach was explored in [63]. The reported there numerical data reveal that taking the interaction effects into account substantially improves an accu- racy of (2.34). Among other FCM-related publications, we mention [26] and similar works where an effective conductivity was estimated up to O(c2) from the “pair-of- inclusions” model. 2.5 Representative Unit Cell Model The third model we consider in our review is so-called “unit cell” model of composite. Its basic idea consists in modeling an actual micro geometry of com- posite by some periodic structure with a unit cell containing several inclusions. It is known in literature as “generalized periodic”, or “quasi-random” model: in what follows, we call it the Representative Unit Cell (RUC) model. This model is advan- tageous in that it allows to simulate the micro structure of composite and, at the same time, take the interactions of inhomogeneities over entire composite space into account accurately. This makes the cell approach appropriate for studying the local ﬁelds and effective properties of high-ﬁlled and strongly heterogeneous composites where the arrangement and interactions between the inclusions substantially affects the overall material behavior. RUC model can be applied to a wide class of compos- ite structures and physical phenomena and, with a rapid progress in the computing technologies, is gaining more and more popularity.
- 18. 114 V. I. Kushch Noteworthy, this model stems from the famous work by Lord Rayleigh [73] who considered “a medium interrupted by spherical obstacles arranged in rectangular order” and has evaluated its effective conductivity by taking into account the dipole, quadrupole and octupole moments of all inclusions. Almost a century later, the complete multipole-type analytical solutions are obtained for three cubic arrays of identical spheres [59, 60, 75, 82, 90]. In a series of more recent papers ([5, 29, 79, 88], among others), the conductivity problem for the random structure composite was treated as a triple-periodic problem with random arrangement of particles in the cubic unit cell. 2.5.1 RUC Geometry The RUC model is essentially the above considered FCM model, periodically con- tinued (replicated) in three orthogonal directions with period a, without overlapping of any two inclusions. In fact, we consider an unbounded solid containing a number N of periodic, equally oriented simple cubic (SC) arrays of inclusions. For a given geometry, any arbitrarily placed, oriented along the principal axes of lattice cube with side length a can be taken as RUC. It contains the centers of exactly N inclu- sions, randomly (but without overlapping) placed within a cell. The inclusions may partially lie outside the cube and, vise versa, a certain part of cube may be occupied by the inclusions which do not belong to the cell, Fig.1a. Equally, one can take the unit cell as a cuboid with curvilinear boundary (but parallel opposite faces): for convenience, we assume with no loss in generality that the cell boundary S0 entirely belongs to the matrix, see Fig.1b. It should be noted that the model problem is formulated and solved for a whole composite bulk rather than for the cube with plane faces. The RUC concept is nothing more than convenient “gadget” for introducing the model geometry and averaging the periodic strain and stress ﬁelds—and we use it for this purpose. We deﬁne geometry of the cell by its side length a and position Rq = Xiqii of qth inclusion center (a) (b) Fig. 1 RUC model of composite
- 19. Multipole Expansion Method in Micromechanics of Composites 115 (q = 1, 2, . . . , N) where ii are the unit axis vectors of the global Cartesian coordinate system Ox1x2x3. Number N can be taken large sufﬁciently to simulate arrangement of disperse phase in composite. We assume the inclusions equally sized, of radius R, and made from the same material, their volume content is c = N 4 3 πR3/a3. In what follows, the parameter Rpq = Rq − Rp is understood as the minimal distance between the inclusions of pth and qth SC arrays. Several methods ([79, 83, 89], among others) have been developed to generate the random structure RUC statistically close to that of actual disordered composite. The generated arrangement of particles, likewise the real composite micro structure, can be characterized by several parameters: packing density, coordination number, radial distribution function, nearest neighbor distance, etc. [7, 83]. Another parameter, often introduced in this type models, is the minimum allowable spacing δmin = minp,q( Rpq /2R−1) [9]. It is also known as impenetrability parameter, in terms of the cherry-pit model [83]. A small positive value is usually assigned to this parameter in order to separate inclusions and thus alleviate analysis of the model problem. 2.5.2 RUC Model Problem The macroscopically uniform temperature ﬁeld in the composite bulk is considered. This means constancy of the volume-averaged, or macroscopic, temperature gradient ∇T and heat ﬂux q vectors. Here and below, f = V −1 V f dV and V = a3 is the cell volume; ∇T is taken as the load governing parameter. In this case, period- icity of geometry results in quasi-periodicity of the temperature ﬁeld and periodicity of the temperature gradient and heat ﬂux: T (r + aii ) = T (r) + a ∇T · ii ; (2.35) ∇T (r + aii ) = ∇T (r) ; q (r + aii ) = q (r) . 2.5.3 Temperature Filed The conditions (2.35) are satisﬁed by taking T in the form T (r) = ∇T ·r+Tdis (r), Tdis being now the periodic disturbance ﬁeld. In the matrix domain, we write it as a sum of linear mean ﬁeld and disturbances form the inﬁnite, periodic arrays of particles: T (0) (r) = G · r + N p=1 T ∗(p) dis (rp), (2.36) The Eq.(2.36) is similar to (2.27), where the single inclusion disturbance terms T (p) dis are replaced with their periodic counterparts given by the sums over all the lattice nodes k = ki ii (−∞ < ki < ∞):
- 20. 116 V. I. Kushch T ∗(p) dis (rp) = k T (p) dis rp + ak , (2.37) In view of (2.37) and (2.27), T ∗(p) dis can be expressed in terms of the periodic harmonic potentials Y∗ ts: T ∗(p) dis (rp) = ∞ t=1 t s=−t A (p) ts Y∗ ts(rp), where Y∗ ts(rp) = k Ys t (rp + ak). (2.38) In fact, this is a direct formal extension of the FCM model when a number of particles becomes inﬁnitely large—and, at the same time, direct extension of the Rayleigh’s [73] approach. For almost a century, the Rayleigh’s solution was ques- tioned due to conditional convergence of (2.38) for t = 1. The limiting process has been legitimized by [59, 82] who resolved the convergence issue of dipole lat- tice sums. An alternate, the generalized periodic functions based approach has been applied by [75, 90]. In [15], the solution has been found in terms of doubly periodic functions, in [88] the RUC problem was solved by the boundary integral method. Not surprisingly, all the mentioned methods give the resulting sets of linear equations consistent with (ωq + 1 + 1 t ) (ωq − 1) (t − s)!(t + s)! Rq 2t+1 A (q) ts + (−1)t+s N p=1 ∞ k=1 k l=−k A (p) kl Y∗ k+t,l−s(Rpq) (2.39) = −δt1 δs0G3 + δs1 (G1 − iG2) − δs,−1 (G1 + iG2) . Among them, the multipole expansion method provides, probably, the most straight- forward and transparent solution procedure. In fact, the system (2.39) is obtained from (2.33) by replacing the matrix coefﬁcients Yl−s k+t (Rpq) with the corresponding lattice sums Y∗ k+t,l−s(Rpq) = k Yl−s k+t Rpq + ak . (2.40) Convergence of the series (2.40) was widely discussed in literature and several fast summation techniques have been developed for them ([17, 59, 88], among others) and we refer there for the details. As would be expected, the Y∗ ts deﬁnition (2.38) for t = 1 also suffers the above- mentioned convergence problem. Indeed, obtained with aid of (2.20) the multipole expansion Y∗ 1s(r) = Ys 1 (r) + ∞ k=0 k l=−k (−1)k+l Y∗ k+1,s−l(R)yl k(r) (2.41)
- 21. Multipole Expansion Method in Micromechanics of Composites 117 also involves the conditionally convergent (“shape-dependent”) dipole lattice sum Y∗ 20(0). McPhedran et al. [59] have argued that the Rayleigh’s [73] result Y∗ 20(0) = 4π/3a3 is consistent with the physics of the problem. Alternatively, Y∗ 1s(r) can be deﬁned by means of periodic fundamental solution S1 [21] given by the triple Fourier series. Speciﬁcally, we deﬁne Y∗ 10 = −D3 (S1) ; Y∗ 11 = −Y∗ 1,−1 = −D2 (S1) ; (2.42) where Di are the differential operators (2.10). It appears that this deﬁnition is equiv- alent to (2.41): differentiation of S1 multipole expansion [21] gives, in our notations, D3 (S1) = −Y0 1 (r) + 4π 3a3 x3 − ∞ k=2 k l=−k (−1)k+l Y∗ k+1,−l(0)yl k(r). (2.43) As expected, exactly the same result follows from the formula (2.41) where y0 1(r) is replaced with x3 and Y∗ 20(0)—with its numerical value, 4π/3a3. 2.5.4 Effective Conductivity The second rank effective conductivity tensor Λ∗ = {λ∗ i j } is deﬁned by (1.1). In order to evaluate λ∗ i j for a given composite, one has to conduct a series of numerical tests, with three different ∇T , and evaluate the macroscopic heat ﬂux it causes. Speciﬁcally, λ∗ i j = − qi for ∇T = ij , so we need an explicit expression of the macroscopic temperature gradient and heat ﬂux corresponding to our temperature solution (2.36). Evaluation of the macroscopic gradient, ∇T is ready. First, we recall that we take the unit cell of RUC with S0 ∈ V0 and, hence, T = T (0) in (1.3). Next, we observe that for the periodic part of solution (2.36) in the boundary points ra ∈ S0 and rb = ra+aij ∈ S0 belonging to the opposite cell faces we have Tdis (rb) = Tdis (ra) whereas the normal unit vector changes the sign: n (rb) = −n (ra). Hence, the integrals of Tdis over the opposite faces cancel each other and the total integral over S0 equals to zero. Integration of the linear part of T (0) is elementary: the gradient theorem yields 1 V S0 (G · r) ndS = 1 V V ∇ (G · r) dV = G. (2.44) Comparison with (1.3) gives the expected ∇T = G provided T obeys (2.35).
- 22. 118 V. I. Kushch This is general result: the derived formula is invariant of the shape, properties andarrangement of inclusions, interfacebondingtypeandshapeof theunit cell. In the subsequent Sections, this equality will be applied without derivation. For q evaluation, we employ the formula (1.9). In the considered here isotropic case, qn (r) = qn (xk) ik = −λ0n, it takes q = − 0 · ∇T − λ0 V N q=1 Sq Rq ∂T (0) ∂rq − T (0) ndS. (2.45) The unit vector n is expressed in terms of surface spherical harmonics as n = χ1 1e2 − 2χ−1 1 e1 + χ0 1e3. whereas the local expansion of the integrand in right hand side of (2.45) is given by Rq ∂T (0) ∂rq − T (0) = ∞ t=0 t s=−t −(2t + 1)A (q) ts (t − s)! Rt+1 q +(t − 1) a (q) ts + c (q) ts Rt q (t + s)! χs t (θq, ϕq). (2.46) Due to orthogonality of the surface spherical harmonics (2.6), the surface integral in (2.45) equals to zero for all terms in Eq.(2.31) with t = 1. Moreover, r ∂ys 1 ∂r = ys 1 and hence only the dipole potentials Ys 1 contribute to (2.45). From here, we get the exact ﬁnite formula involving only the dipole moments of the disturbance ﬁeld, A (q) 1s : q λ0 = −G + 4π a3 N q=1 Re 2A (q) 11 e1 + A (q) 10 e3 . (2.47) In view of (2.39), the coefﬁcients A (q) ts are linearly proportional to G: λ0 4π a3 N q=1 Re 2A (q) 11 e1 + A (q) 10 e3 = δ · G. (2.48) The components of the δ tensor are found by solving Eq.(2.39) for G = ij . These equations, together with Eq.(1.1), provide evaluation of the effective conductivity tensor as ∗ = 0 + δ . (2.49)
- 23. Multipole Expansion Method in Micromechanics of Composites 119 3 Composite with Spherical Inclusions: Elasticity Problem 3.1 Background Theory 3.1.1 Vectorial Spherical Harmonics Vectorial spherical harmonics S (i) ts = S (i) ts (θ, ϕ) are deﬁned as [64] S(1) ts = eθ ∂ ∂θ χs t + eϕ sin θ ∂ ∂ϕ χs t ; (3.1) S (2) ts = eθ sin θ ∂ ∂ϕ χs t − eϕ ∂ ∂θ χs t ; S (3) ts = er χs t (t ≥ 0, |s| ≤ t). The functions (3.1) constitute a complete and orthogonal on sphere set of vectorial harmonics with the orthogonality properties given by 1 S S S (i) ts · S ( j) kl dS = α (i) ts δtkδslδi j , (3.2) where α(1) ts = α(2) ts = t(t+1) αts and α(3) ts = αts given by (2.6). Also, these functions possess remarkable differential r∇ · S (1) ts = −t(t + 1)χs t ; ∇ · S (2) ts = 0; r∇ · S (1) ts = 2χs t ; (3.3) r∇ × S (1) ts = −S (2) ts ; r∇ × S (2) ts = S (1) ts + t(t + 1)S (3) ts ; r∇ × S (3) ts = S (2) ts ; and algebraic er × S(1) ts = −S(2) ts ; er × S(2) ts = S(1) ts ; er × S(3) ts = 0; (3.4) properties. In the vectorial—including elasticity—problems, the functions (3.1) play the same role as the surface harmonics (2.5) in the scalar problems. With aid of (3.3), (3.4), separation of variables in the vectorial harmonic Δf = 0 and bihar- monic ΔΔg = 0 equations is straightforward [17, 30] and yields the correspond- ing countable sets of partial solutions—vectorial solid harmonics and biharmonics, respectively. 3.1.2 Partial Solutions of Lame Equation The said above holds true for the Lame equation
- 24. 120 V. I. Kushch 2(1 − ν) (1 − 2ν) ∇(∇ · u) − ∇ × ∇ × u = 0 (3.5) being the particular case of vectorial biharmonic equation. In (3.5), u is the dis- placement vector and ν is the Poisson ratio. The regular partial solutions of (3.5) u(i) ts = u(i) ts (r) are deﬁned as [30] u (1) ts = rt−1 (t + s)! S (1) ts + tS (3) ts , u (2) ts = − rt (t + 1)(t + s)! S (2) ts , (3.6) u (3) ts = rt+1 (t + s)! βt S (1) ts + γt S (3) ts , βt = t + 5 − 4ν (t + 1)(2t + 3) , γt = t − 2 + 4ν (2t + 3) . The singular (inﬁnitely growing at r → 0 and vanishing at inﬁnity) functions U (i) ts are given by U (i) ts = u (i) −(t+1), s, with the relations S (i) −t−1,s = (t −s)!(−t −1+s)!S (i) ts taken into account. The functions u(i) ts (r) and U(i) ts (r) are the vectorial counterparts of scalar solid harmonics (2.4). At the spherical surface r = R, the traction vector Tn = σ · n can be written as 1 2μ Tr (u) = ν 1 − 2ν er (∇ · u) + ∂ ∂r u + 1 2 er × (∇ × u) , (3.7) μ being the shear modulus. For the vectorial partial solutions (3.6), it yields [30] 1 2μ Tr (u (1) ts ) = (t − 1) r u (1) ts ; 1 2μ Tr (u (2) ts ) = (t − 1) 2r u (2) ts ; (3.8) 1 2μ Tr (u(3) ts ) = rt (t + s)! bt S(1) ts + gt S(3) ts ; where bt = (t + 1)βt − 2(1 − ν)/(t + 1) and gt = (t + 1)γt − 2ν. In view of (3.6), representation of Tr (u (i) ts ) in terms of vectorial spherical harmonics (3.1) is obvious. The total force T and moment M acting on the spherical surface S of radius R are given by the formulas T = Sr Tr dS, M = Sr r × Tr dS, (3.9) It is straightforward to show that T = M = 0 for all the regular functions u (i) ts . Among the singular solutions U (i) ts , we have exactly three functions with non-zero resultant force T: T U (3) 10 = 16μπ(ν − 1)e3; T U (3) 11 = −T U (3) 1,−1 = 32μπ(ν − 1)e1. (3.10)
- 25. Multipole Expansion Method in Micromechanics of Composites 121 By analogy with Y0 0 , U (3) 1s can be regarded as the vectorial monopoles. The resultant moment is zero for all the partial solutions but U (2) 1s for which we get M U (2) 10 = −8μπe3; M U (2) 11 = M U (2) 1,−1 = −16μπe1. (3.11) 3.2 Single Inclusion Problem In the elasticity problem, we deal with the vectorial displacement ﬁeld u (u = u(0) in a matrix, u = u(1) in the spherical inclusion of radius R) satisfying (3.5). On the interface S, perfect mechanical contact is assumed: [[u]] = 0; [[Tr (u)]] = 0; (3.12) where Tr is given by (3.7). The elastic moduli are (μ0, ν0) for matrix material and (μ1, ν1) for inclusion, the non-uniform displacement far ﬁeld u f ar is taken as the load governing parameter. 3.2.1 Series Solution The displacement in the inclusion u(1) is ﬁnite and so allows expansion into a series over the regular solutions u (i) ts (r) (3.6): u(1) (r) = i,t,s d (i) ts u (i) ts (r) ⎛ ⎝ i,t,s = 3 i=1 ∞ t=0 t s=−t ⎞ ⎠ , (3.13) where d (i) ts are the unknown constants. The components of the displacement vector are real quantities, so the property u(i) t,−s = (−1)su(i) ts gives d(i) t,−s = (−1)sd(i) ts . In the matrix domain, we write u(0) = u f ar +udis, where the disturbance part udis(r) → 0 with r → ∞ and hence can be written in terms of the singular solutions U (i) ts only: u(0) (r) = u f ar (r) + i,t,s A (i) ts U (i) ts (r) (3.14) where A (i) ts are the unknown coefﬁcients. By analogy with (2.14), the series term is thought as the multipole expansion of udis.
- 26. 122 V. I. Kushch 3.2.2 Far Field Expansion Due to regularity of u f ar , we can expand it into a series (3.13) with coefﬁcients c ( j) ts . With aid of (3.6), we express u f ar at r = R in terms of vectorial spherical harmonics (3.1) u f ar (r) = j,t,s c (i) ts u (i) ts (r) = j,t,s c (i) ts (t + s)! 3 i=1 U M i j t (R, ν0)S (i) ts (θ, ϕ) (3.15) where UMt is a (3 × 3) matrix of the form UMt (r, ν) = U M i j t (r, ν) = rt−1 ⎧ ⎪⎨ ⎪⎩ 1 0 r2βt (ν) 0 − r t+1 0 t 0 r2γt (ν) ⎫ ⎪⎬ ⎪⎭ . (3.16) Now, we multiply (3.15) by S(i) ts and integrate the left-hand side (either analytically or numerically) over the interface S. In view of (3.2), analytical integration of the right-hand side of (3.15) is trivial and yields J(i) ts = (t + s)! 4πR2α(i) ts S u f ar · S(i) ts dS = 3 j=1 U M i j t (R, ν0) c ( j) ts (3.17) From the above equation, we get the expansion coefﬁcients in matrix-vector form as cts = UMt (R, ν0)−1 Jts (3.18) where cts = c (i) ts T and Jts = J (i) ts T . In the particular case of linear u f ar = E · r, where E = Ei j is the uniform far-ﬁeld strain tensor, the explicit analytical expressions for the expansion coefﬁcients are c (3) 00 = (E11 + E+ 22 E33) 3γ0(ν0) , c (1) 20 = (2E33 − E11 − E22) 3 , c (1) 21 = E13 − i E23, c (1) 22 = E11 − E22 − 2i E12; (3.19) c (i) 2,−s = (−1)sc (i) 2s and all other c (i) ts are equal to zero. 3.2.3 Resolving Equations Now, we substitute (3.13) and (3.14) into the ﬁrst condition of (3.12) and use the orthogonality of S (i) ts to reduce it to a set of linear algebraic equations, written in matrix form as (UGt = UM−(t+1))
- 27. Multipole Expansion Method in Micromechanics of Composites 123 (t − s)!(t + s)!UGt (R, ν0) · Ats + UMt (R, ν0) · cts = UMt (R, ν1) · dts. (3.20) The second, traction continuity condition gives us another set of equations: (t − s)!(t + s)!TGt (R, ν0) · Ats + TMt (R, ν0) · cts = ωTMt (R, ν1) · dts, (3.21) where ω = μ1/μ0. In (3.21), the TM is (3 × 3) matrix T Mt (r, ν) = T M i j t (r, ν) = rt−2 ⎧ ⎪⎨ ⎪⎩ t − 1 0 r2bt (ν) 0 −r(t−1) 2(t+1) 0 t(t − 1) 0 r2gt (ν) ⎫ ⎪⎬ ⎪⎭ . (3.22) where gt and bt are deﬁned by (3.8); TGt = TM−(t+1), Ats = A (i) ts T and dts = d (i) ts T . For all indices t ≥ 0 and |s| ≤ t, the coefﬁcients Ats and dts can be found from linear system (3.20), (3.21). For computational purposes, it is advisable to eliminate dts from there and obtain the equations containing the unknowns Ats only: (t − s)!(t + s)!(RMt )−1 RGt · Ats = −cts, (3.23) where RGt = ω [UMt (R, ν1)]−1 UGt (R, ν0) − [TMt (R, ν1)]−1 TGt (R, ν0), RMt = ω [UMt (R, ν1)]−1 UMt (R, ν0) − [TMt (R, ν1)]−1 TMt (R, ν0). (3.24) This transformation is optional for a single inclusion problem but can be rather useful for the multiple inclusion problems where the total number of unknowns becomes very large. The equations with t = 0 and t = 1 deserve extra attention. First, we note that U (2) 00 = U (3) 00 ≡ 0 and so we have only one equation (instead of three) in (3.23). It can be resolved easily to get 1 R3 4μ0 + 3k1 3k0 − 3k1 a (1) 00 = −c (3) 00 (3.25) where the relation a0 γ0 = 3k 2μ (k being the bulk modulus) is taken into consideration. Noteworthy, Eq.(3.25) gives solution of the single inclusion problem in the case of equiaxial far tension: E11 = E22 = E33. For t = 1, the ﬁrst two columns of the matrix TMt (3.22) become zero: also, a1+2b1 = 0. From (3.23), we get immediately A (2) 1s = A (3) 1s = 0. The solution we obtain is complete and valid for any non-uniform far ﬁeld. For any polynomial far ﬁeld of order tmax, this solution is exact and conservative, i.e., is given by the ﬁnite number of terms with t ≤ tmax. For example, in the
- 28. 124 V. I. Kushch Eshelby-type problem, the expansion coefﬁcients with t ≤ 2 are nonzero only. The solution procedure is straightforward and remarkably simple as compared with the scalar harmonics-based approach (see, e.g., [72]). In fact, use of the vectorial spher- ical harmonics makes the effort of solving the vectorial boundary value problems comparable to that of solving scalar boundary value problems. Also, solution is writ- ten in the compact matrix-vector form, readily implemented by means of standard computer algebra. 3.3 Re-Expansion Formulas The re-expansions of the vectorial solutions U (i) ts and u (i) ts (3.5) are [30]: singular-to- regular (S2R) U (i) ts (r + R) = 3 j=1 ∞ k=0 k l=−k (−1)k+l η (i)( j) tksl (R)u ( j) kl (r), r < R ; (3.26) where η (i)( j) tksl = 0, j > l; η (1)(1) tksl = η (2)(2) tksl = η (3)(3) tksl = Ys−l t+k ; (3.27) η(2)(1) tksl = i s t + l k Ys−l t+k−1; η(3)(2) tksl = −4 (1 − ν) η(2)(1) tksl , k ≥ 1; η (3)(1) tksl = l k η (3)(2) t,k−1,sl − Zs−l t+k − Ys−l t+k−2 × (t + k − 1)2 − (s − l)2 2t + 2k − 1 + C−(t+1),s + Ck−2,l ; regular-to-regular (S2R): u (i) ts (r + R) = i j=1 t+i− j k=0 k l=−k (−1)k+l ν (i)( j) tksl (R)u ( j) kl (r); (3.28) where ν (i)( j) tksl = 0, j > l; ν (1)(1) tksl = ν (2)(2) tksl = ν (3)(3) tksl = ys−l t−k; (3.29) ν(2)(1) tksl = i s t + 1 − l k ys−l t−k+1; ν(3)(2) tksl = −4 (1 − ν) ν(2)(1) tksl ;
- 29. Multipole Expansion Method in Micromechanics of Composites 125 ν(3)(1) tksl = l k ν(3)(2) t,k−1,sl − zs−l t−k − ys−l t−k+2 (t − k + 2)2 − (s − l)2 2t − 2k + 3 − Cts + Ck−2,l ; and singular-to-singular (S2S): U (i) ts (r + R) = 3 j=1 ∞ k=t−i+ j k l=−k (−1)t+k+s+l μ (i)( j) tksl (R)U ( j) kl (r), r > R ; (3.30) where μ (i)( j) tksl = 0, j > l; μ (1)(1) tksl = μ (2)(2) tksl = μ (3)(3) tksl = ys−l k−t ; (3.31) μ (2)(1) tksl = i s t − l k + 1 ys−l k−t+1; μ (3)(2) tksl = −4 (1 − ν) μ (2)(1) tksl ; μ (3)(1) tksl = − l k + 1 μ (3)(2) t,k+1,sl + zs−l k−t − ys−l k−t+2 (t + k − 2)2 − (s − l)2 2k − 2t + 3 + C−(t+1),s + C−(k+3),l . In these formulas, Zs t = r2 2t−1 Ys t and zs t = r2 2t+3 ys t are the singular and regular, respectively, scalar solid biharmonics and Cts = (t + 1)2 − s2 βt . These formulas are the vectorial counterparts of (2.20)–(2.22): being combined with FMM [19] scheme, they provide the fast multipole solution algorithm for elastic interactions in the multiple inclusion problem. For the Stokes interactions in suspension of spherical particles, similar work is done in [77]. 3.4 FCM Analysis of the FCM elasticity problem is analogous to that of conductivity, so we outline the procedure and formulas. For simplicity sake, we assume the far displace- ment ﬁeld to be linear: u f ar = E · r. 3.4.1 Direct (Superposition) Sum We use the superposition principle to write
- 30. 126 V. I. Kushch u(0) (r) = u f ar (r) + N p=1 u (p) dis(rp), (3.32) where u (p) dis(r) = i,t,s A (i)(p) ts U (i) ts (r) (3.33) is the displacement disturbance ﬁeld caused by pth inclusion: u (p) dis(rp) → 0 as rp → ∞. 3.4.2 Local Expansion Sum In a vicinity of Oq, the following expansions are valid: u f ar (r) = u f ar (Rq) + u f ar (rq) = ε∞ · Rq + ∞ t=0 t s=−t c (i) ts u (i) ts (rq), (3.34) where c (i) tst are given by (3.19). Displacement u (q) dis in (3.32) is written in the local coordinate system of the qth inhomogeneity and ready for use. For p = q, we apply the re-expansion formula (3.26) to get u(0) (r) = ε∞ · Rq + i,t,s A (i)(q) ts U (i) ts (rq) + a (i)(q) ts u (i) ts (rq) , (3.35) where a (i)(q) ts = N p=q j,k,l (−1)k+l A ( j)(p) kl η ( j)(i) ktls (Rpq). (3.36) In matrix form, a (q) ts = N p=q k,l ηktls(Rpq) T · A (p) kl (3.37) where A (q) ts = A (i)(q) ts T , a (q) ts = a (i)(q) ts T and ηtksl = (−1)k+l η (i)( j) tksl . 3.4.3 Inﬁnite System of Linear Equations With the displacement within qth inhomogeneity represented by the series (3.13) with coefﬁcients d (q) ts d (i)(q) ts T , we come to the above considered single inclusion problem. The resulting inﬁnite system of linear equations has the form
- 31. Multipole Expansion Method in Micromechanics of Composites 127 (t−s)!(t+s)!(RM (q) t )−1 RG (q) t ·A (q) ts + N p=q k,l ηktls(Rpq) T ·A (p) kl = −cts, (3.38) where RM (q) t = RMt (Rq, ν0, νq) and RG (q) t = RGt (Rq, ν0, νq) are given by (3.24). Likewise (2.33), this system can be solved by the truncation method. Again, the obtained solution is straightforward and remarkably simple: see, for comparison, solution of two-sphere problem [8]. This approach enables an efﬁcient analytical solution to a wide class of 3D elasticity problems for multiple-connected domains withspherical boundaries, inparticular, studyof elasticinteractions between the spherical nano inclusions with Gurtin-Murdoch type interfaces [54]. 3.4.4 FCM and Effective Elastic Moduli We deﬁne, by analogy with FCM conductivity problem, an equivalent inclusion radius as R3 ef f = N/c, c being a volume fraction of inclusions, and compare, in spirit of Maxwell’s approach, an asymptotic behavior of disturbances caused by the ﬁnite cluster of inclusions and “equivalent” inclusion. To this end, we apply the (S2S) re-expansion (3.30), giving us for r > maxp Rp N p=1 u (p) dis(r) = i,t,s e (i) ts U (i) ts (r), (3.39) where ets = N p=1 k,l μktls(−Rp) T · A (p) kl (3.40) and μtksl = μ (i)( j) tksl . Now, we equate ets given by (3.40) to ats in (3.23) to determine the effective moduli of composite. Considering the equiaxial far tension ε∞ 11 = ε∞ 22 = ε∞ 33 gives us, in view of (3.25), an expression for the effective bulk modulus kef f kef f = 3k0 + 4μ0 c A (1) 00 3 1 − c A (1) 00 , (3.41) where A(1) 00 = 1 N N p=1 A (1)(p) 00 is the mean dipole moment. In the case we neglect interactions between the inclusions, (3.41) reduces to the mechanical counterpart of the original Maxwell’s formula (e.g., [58]).
- 32. 128 V. I. Kushch 3.5 RUC The stress ﬁeld in the composite bulk is assumed to be macroscopically uniform, which means constancy of the macroscopic strain ε and stress σ tensors. We take ε = E as input (governing) load parameter. Alike the conductivity problem, periodic geometry of composite results in quasi-periodicity of the displacement ﬁeld and periodicity of the strain and stress ﬁelds: u (r + aii ) = u (r) + aE · ii ; (3.42) ε (r + aii ) = ε (r) ; σ (r + aii ) = σ (r) . 3.5.1 Displacement Field The conditions (3.42) are fulﬁlled by taking u (r) = ε · r + udis (r), where udis is the periodic disturbance displacement ﬁeld. In the matrix domain, we write u in the form analogous to (2.36): u(0) (r) = E · r + N p=1 u ∗(p) dis (rp), (3.43) where u ∗(p) dis (rp) = k u (p) dis rp + ak (3.44) and u (p) dis(r) = i,t,s A (i)(p) ts U (i) ts (r). (3.45) Again, by analogy with (2.38), u ∗(p) dis can be expressed in terms of the periodic functions U ∗(i) ts [30]: u ∗(p) dis (rp) = ∞ i,ts A (p) ts U ∗(i) ts (rp), U ∗(i) ts (rp) = k U (i) ts (rp + ak). (3.46) An alternate, mathematically equivalent set of vectorial periodic functions have been written [76] in terms of fundamental periodic solutions [21]. The resulting linear system closely resembles that for FCM (3.38):
- 33. Multipole Expansion Method in Micromechanics of Composites 129 (t−s)!(t+s)!(RM (q) t )−1 RG (q) t ·A (q) ts + N p=1 k,l η∗ ktls(Rpq) T ·A (p) kl = −cts, (3.47) where c (i) ts are given by (3.19). The matrix coefﬁcients η∗ ktls(Rpq) are the lattice sums of corresponding expansion coefﬁcients η∗ ktls(Rpq) (3.27). Their evaluation is mostly based on the relevant results for scalar potential (2.40). The only new feature here is the biharmonic lattice sum Z∗ k+t,l−s(Rpq) = k Zl−s k+t Rpq + ak ; (3.48) for Zs t deﬁnition, see Sect.3.3. This sum closely relates the fundamental solution S2 in [21]: its evaluation with aid of Evald’s technique is discussed there. 3.5.2 Effective Stiffness Tensor The fourth rank effective elastic stiffness tensor C∗ = C∗ i jkl is deﬁned by (1.10). In order to evaluate C∗ i jkl for a given geometry of composite, one must conduct a series of numerical tests with different macro strains Ei j and evaluate the macro stress σ Eq.(1.12). Speciﬁcally, C∗ i jkl = σi j for εmn = δmkδnl. For this purpose, we need the explicit expressions of average strain and stress corresponding to our displacement solution. Evaluation of the macroscopic strain tensor, ε is elementary. First, we recall that we have taken RUC with S0 ∈ V0, so u = u(0) in (1.12). Next, we observe that for the periodic part of solution in the boundary points ra ∈ S0 and rb = ra + aij ∈ S0 belonging to the opposite cell faces we have udis (rb) = udis (ra) whereas the normal unit vector changes the sign: n (rb) = −n (ra). Hence, the integrals of udis over the opposite faces cancel each other and the total integral over S0 equals to zero. Integration of the linear part of u(0) is elementary: the divergence theorem gives the expected ε = E. A suitable for our purpose expression of the macroscopic stress tensor σ is given by (1.13). Noteworthy, surface integration in (1.13) is greatly simpliﬁed by taking u(i) ts as a trial displacement vector u . It follows from (3.19) that u(3) 00 and u(1) 2s are the linear function of coordinates. For example, u (3) 00 = rγ0S (3) 00 = γ0r =γ0ukk; also, Tn(u (3) 00 ) = 3k r u (3) 00 , k being the bulk modulus. We get from Eq.(1.13) σii = C(0) iikk εkk + 1 V N q=1 Sq Tn(u(0) ) − 3k0 r u(0) · u (3) 00 γ0 dS. (3.49) Now, we put here the local expansion of u(0) given by Eq.(3.35) and the analogous expansion of Tn u(0) :
- 34. 130 V. I. Kushch Tn u(0) (rq) = i,t,s A (i)(q) ts Tn U (i) ts (rq) + a (i)(q) ts + c (i) ts Tn u (i) ts (rq) . (3.50) For the explicit expression of Tn(U (i) ts ) and Tn(u (i) ts ) in terms of vectorial spherical harmonics S (i) ts , see [54]. By taking orthogonality of these harmonics on the sphere into account we ﬁnd that the only function giving non-zero contribution to the integral in (3.49) is U (1) 00 = − 2 r2 S (3) 00 for which Tn U (1) 00 = −4μ r U (1) 00 = 8μ r3 S (3) 00 . Thus, we obtain Sq Tn(u(0) ) − 3k0 r u(0) · u (3) 00 γ0 dS = A (1)(q) 00 2 R2 (4μ0 + 3k0) Sq S (3) 00 · S (3) 00 dS = 8π (4μ0 + 3k0) A (1)(q) 00 . By using in the same way the (simple shear mode) functions u(1) 20 = u33 − (u11 + u22)/2; u(1) 21 = u13 + u31 /2 + i(u23 + u32)/2; u(1) 22 = u11 − u22 /4 + i u12 + u21 /4; for which Tr (u (1) 2s ) = 2μ r u (1) 2s , we come to the ﬁnite exact formulas S11 + S22 + S33 = (1 + ν0) (1 − 2ν0) (E11 + E22 + E33) + 12π a3 (1 − ν0) (1 − 2ν0) N q=1 A (1)(q) 00 ; 2S33 − S11 − S22 = 2E33 − E11 − E22 − 16π a3 (1 − ν0) N q=1 A (3)(q) 20 ; S11 − S22 − 2iS12 = E11 − E22 − 2iE12 − 32π a3 (1 − ν0) N q=1 A (3)(q) 22 ; S13 − iS23 = E13 − iE23 − 8π a3 (1 − ν0) N q=1 A (3)(q) 21 . (3.51) where Si j = σi j /2μ0. The coefﬁcients A (i)(q) ts are linearly proportional to E. The σi j are uniquely determined from Eqs.(3.47, 3.51) for Ekl given and, thus, these equations together with (1.10) are sufﬁcient for evaluation of the effective stiffness tensor, C∗. (3.51) involves only the expansion coefﬁcients A (i)(q) i−1,s which can be regarded as the dipole moments. The effective elastic moduli of composite with simple cubic array of spherical inclusions have been found by [31, 76], for the RUC type structure—by [17, 78].
- 35. Multipole Expansion Method in Micromechanics of Composites 131 4 Composite with Spheroidal Inclusions 4.1 Scalar Spheroidal Solid Harmonics The spheroidal coordinates (ξ, η, ϕ) relate the Cartesian coordinates (x1, x2, x3) by [23] x1 + ix2 = dξη exp(iϕ), x3 = dξη, (4.1) where ξ 2 = ξ2 − 1, η2 = 1 − η2 (1 ≤ ξ < ∞, −1 ≤ η ≤ 1, 0 ≤ ϕ < 2π). (4.2) At Re(d) > 0, the formulas (4.1) and (4.2) deﬁne a family of confocal prolate spheroids with inter-foci distance 2d: to be speciﬁc, we expose all the theory for this case. In the case of oblate spheroid, one must replace ξ with iξ and d with (−id) in these and all following formulas. For d → 0 and dξ → r, the spheroidal coordinates system degenerates into spherical one, with η → cos θ. Separation of variables in Laplace equation in spheroidal coordinates gives us the sets of partial solutions, or solid spheroidal harmonics: regular f s t (r, d) = P−s t (ξ)χs t (η, ϕ) = (t − s)! (t + s)! Ps t (ξ)χs t (η, ϕ) (4.3) and irregular Fs t (r, d) = Q−s t (ξ)χs t (η, ϕ) = (t − s)! (t + s)! Qs t (ξ)χs t (η, ϕ) (4.4) Here, Qs t are the associate Legendre’s functions of second kind [23]. The functions (4.3) and (4.4) obey the properties analogous to (2.7). The functions Fs t → 0 with r → ∞ and, by analogy with Ys t , can be regarded as spheroidal multipole poten- tials. We mention the multipole type re-expansions between Ys t and Fs t [13] which, in our notations, take the form Fs t (r, d) = (−1)s ∞ k=t K(1) tk (d)Ys k (r) ( r > d); (4.5) Ys t (r) = (−1)s ∞ k=t K (2) tk (d)Fs k (r, d);
- 36. 132 V. I. Kushch where K (1) tk (d) = d 2 k+1 √ π Γ k−t 2 + 1 Γ k+t 2 + 3 2 , (4.6) K (2) tk (d) = 2 d k+1 (−1)(k−t)/2 k + 1 2 Γ k+t 2 + 1 2 √ πΓ k−t 2 + 1 for (t−k) even and equal to zero otherwise. The analogous relations are also available for the regular solid harmonics, ys t and f s t [39]. 4.2 Single Inclusion: Conductivity Problem Let an unbounded solid contains a single prolate spheroidal inclusion with boundary deﬁned by ξ = ξ0. The matrix-inclusion thermal contact obeys the conditions (2.9) where qr is replaced with qξ = −λ∇T ·eξ = d−1(ξ 2 −η2)−1/2∂T/∂ξ. The solution ﬂow is quite analogous to that for the spherical inclusion, so we outline it brieﬂy. 4.2.1 Series Solution The temperature ﬁeld inside the inclusion is given by a series T (1) (r) = ∞ t=0 t s=−t dts f s t (r, d). (4.7) The temperature ﬁeld outside the inclusion is a sum of far and disturbance ﬁelds: T (0) (r) = Tf ar (r) + Tdis(r), Tdis(r) = ∞ t=1 t s=−t Ats Fs t (r, d). (4.8) The second term in (4.8) can be thought as the spheroidal multipole expansion of the disturbance ﬁeld Tdis. Noteworthy, at some distance from inclusion (namely, where r > d) it can be also expanded, by applying formula (4.5), over the spherical multipoles Ys t . The Tf ar series expansion in a vicinity of inclusion is analogous to (4.7). In view of (2.6), the cts coefﬁcients are equal to cts = (2t + 1) 4πPs t (ξ0) 2π 0 dϕ 1 −1 Tf ar χs t (η, ϕ) dη. (4.9)
- 37. Multipole Expansion Method in Micromechanics of Composites 133 4.2.2 Resolving Equations The temperature continuity at ξ = ξ0 gives, in view of χs t (η, ϕ) orthogonality (2.6), a set of linear algebraic equations Qs t (ξ0)Ats + Ps t (ξ0)cts = Ps t (ξ0)dts. (4.10) The second, normal ﬂux continuity condition gives us also Q s t (ξ0)Ats + P s t (ξ0)cts = ωP s t (ξ0)dts, (4.11) where ω = λ1/λ0 and stroke means derivative with respect to argument. The ﬁnal formula for the coefﬁcients Ats is 1 (ω − 1) ω Qs t (ξ0) Ps t (ξ0) − Q s t (ξ0) P s t (ξ0) Ats = −cts. (4.12) 4.3 Re-expansion Formulas We deﬁne the inclusion-related local coordinate system in a way that coordinate surface coincides with the surface of inclusion. Spheroidal shape of inclusion dictates the origin and, in contrast to spherical case, orientation of this system. A general transformation of coordinates can be splitted into a sum of translation and rotation, i.e. r1 = R + O · r2 where O is a symmetrical positively deﬁnite matrix with det O = 1. Analogously, the general re-expansion formula is given by superposition of two more simple formulas, one written for translation and another—for rotation. 4.3.1 Translation Inthecaseofco-axial(O = I)coordinatesystems(d1, ξ1, η1, ϕ1)and(d2, ξ2, η2, ϕ2) centered at the points O1 and O2, respectively, the re-expansion formulas (addition theorems) of three kinds for the spheroidal solid harmonics are [32, 35, 37]: Fs t (r1, d1) = ∞ k=0 k l=−k ηtk,s−l (R, d1, d2) f l k (r2, d2) ; (4.13) f s t (r1, d1) = t k=0 k l=−k μtk,s−l (R, d1, d2) f l k (r2, d2) ; (4.14) Fs t (r1, d1) = ∞ k=t k l=−k νtk,s−l (R, d1, d2) Fl k (r2, d2) . (4.15)
- 38. 134 V. I. Kushch A simple way to derive these formulas consists in combining the formulas (4.5), (4.6) with the relevant re-expansions for spherical harmonics (2.20)–(2.22). Say, for (4.13) this procedure yields η (1) tks = atk ∞ r=0 d1 2 2r Mtkr (d1, d2) Ys t+k+2r (R) , (4.16) where atk = (−1)k+l π k + 1 2 d1 2 t+1 d2 2 k , (4.17) Mtkr = r j=0 (d2/d1)2 j j!(r − j)!Γ (t + r − j + 3/2) Γ (k + j + 3/2) (4.18) and Γ (z) is the gamma-function [1]. For d1 = d2, this expression reduces to Mtkr = (t + k + r + 2)r r! Γ (t + r + 3/2) Γ (k + r + 3/2) , (4.19) where (n)m is the Pochhammer’s symbol. Derived this way the coefﬁcients in (4.14) and (4.15) are μ (1) tks = k + 1 2 d1 2 −t d2 2 k σ r=0 d1 2 2r ys t−k−2r (R) (4.20) × r j=0 (−1)r− j Γ (t + j − r + 1/2) (d2/d1)2 j j!(r − j)! Γ (k + j + 3/2) and ν (1) tks = k + 1 2 d1 2 t+1 d2 2 −(k+1) σ r=0 d1 2 2r ys k−t−2r (R) (4.21) × r j=0 (−1)j Γ (k − j + 1/2) (d2/d1)2 j j!(r − j)! Γ (t + r − j + 3/2) , respectively. Here, σ = |t − k| − |s|. They are consistent with the formulas reported by [13]. It appears, however, that formula (4.13) with coefﬁcients (4.16) is valid only for R > d1 + d2; this fact is due to the geometry restriction in (4.5) and (2.20) used for derivation. A general, geometrical restrictions-free expression [32] is
- 39. Multipole Expansion Method in Micromechanics of Composites 135 η (2) tks = atk √ π 2 d3 t+k+1 ∞ r=0 Fs t+k+2r (R, d3) t + k + 2r + 1 2 (4.22) × r j=0 (−1)r− j (r − j)! d1 d3 2 j Γ (t + k + r + j + 1/2) Mtkj (d1, d2) The series (4.13) with coefﬁcients (4.22) for d3 > d1 converges in all points inside the spheroid ξ2 = ξ20 with the center at a point O2 and inter-foci distance 2d2 if point O1 lies outside the spheroid with semiaxes d2ξ20 and d2ξ20 + d1 (ξ12 > ξ0 12). Here, ξ0 12 = cosh arctanh d2ξ20 d2ξ20 + d1 (4.23) where (d12, ξ12, η12, ϕ12) are spheroidal coordinates of vector R in a system with origin in the point O2 and d12 = (d2ξ20 + d1) /ξ0 12. This is condition of non- intersecting the spheroidal surface ξ2 = ξ20 and inﬁnitely thin spheroid with inter- foci distance 2d1 centered at point O1 and holds true for any two non-intersecting spheroids of ﬁnite size. In the case R > d1 + d2, both the representations, η (1) tk,s−l and η (2) tk,s−l are valid and using the simpler expression (4.16) is preferable. For R < d1 + d2, η (1) tk,s−l diverges and η (2) tk,s−l should be used instead. Noteworthy, convergence rate of (4.23) is geometry-dependent and the numerical difﬁculties may arise, e.g., for the closely placed very elongated spheroids. In this situation, using the numerical integration formula ηtk,s−l = (2t + 1) 4πPl k(ξ20) 2π 0 dϕ2 1 −1 Fs t (r + R, d1) χl k(η2, ϕ2) dη2 (4.24) analogous to (4.9) would be the most appropriate option. 4.3.2 Rotation The re-expansion of spheroidal solid harmonics (4.3) and (4.4) due to the rotation of the coordinate system (R = 0, d1 = d2 = d) is determined by f s t (r1, d) = t k=0 k l=−k f l k (r2, d) (−1)s+l k + 1 2 (4.25) × ∞ r=k (−1) t−r 2 Γ t+r 2 + 1 2 t−r 2 ! r−k 2 !Γ r+k 2 + 3 2 (r − l)!(r + l)! (r − s)!(r + s)! Sr−s,r−l 2r (w);
- 40. 136 V. I. Kushch Fs t (r1, d) = ∞ k=t k l=−k Fl k (r, d) (−1)s+l k + 1 2 (4.26) × ∞ r=k (−1) t−r 2 Γ t+r 2 + 1 2 r−t 2 ! k−r 2 !Γ r+t 2 + 3 2 Sr−s,r−l 2r (w); where primes over the sums denote that they contain only terms with even (t − k) and (t − r). Also, Ss,l t are the spherical harmonics [3] in four-dimensional space, w = wi is the unit four-dimensional vector determining uniquely the rotation matrix O = ⎛ ⎜ ⎝ w2 2 − w2 1 − w2 3 + w2 4 2 (w2w3 − w1w4) 2 (w1w2 + w3w4) 2 (w2w3 + w1w4) w2 3 − w2 1 − w2 2 + w2 4 2 (w1w3 − w2w4) 2 (w1w2 − w3w4) 2 (w1w3 + w2w4) w2 1 − w2 2 − w2 3 + w2 4 ⎞ ⎟ ⎠ . (4.27) These results are similar to those derived by [13]. Coupled with (4.13)–(4.15), they provide the representation of spheroidal solid harmonics in any arbitrary positioned and oriented coordinate system and thus form a theoretical basis of solving the poten- tial theory problems for multiply connected domains with spheroidal boundaries by the Multipole Expansion Method. 4.4 FCM Let consider an unbounded solid containing N spheroidal inclusions of conductivity λq centered in the points Oq. Geometry of qth inclusion (q = 1, 2, . . . , N) is deﬁned by two numbers: ξ0 = ξq0 and d = dq. Its position and orientation are given by the vector Rq, and matrix Oq, respectively. The local Cartesian (x1q, x2q, x3q) and spheroidal (dq, ξq, ηq, ϕq) coordinates are related by (4.1); r = Rq + Oq · rq. The linear far ﬁeld Tf ar = G · r is prescribed. Temperature in the matrix solid is given by the superposition sum (2.27), where the disturbance ﬁeld caused by pth inclusion is written now in terms of spheroidal multipoles: T (p) dis (rp) = ∞ t=1 t s=−t A (p) ts Fs t (rp, dp). (4.28) In a vicinity of Oq, the following expansions are valid: Tf ar (rq) = ∞ t=0 t s=−t c (q) ts f s t (rq), (4.29)
- 41. Multipole Expansion Method in Micromechanics of Composites 137 where c (q) 00 = G·Rq, c (q) 10 = Gi Oi3qdq, c (q) 11 = 2dq Gi (Oi1q −iOi2q), c (q) 1,−1 = −c (q) 11 and c (q) ts = 0 otherwise. The term T (q) dis is already written in qth basis; for p = q, we apply the re-expansion formulas for irregular solid harmonics to get T (p) dis (rq) = ∞ t=0 t s=−t a (q) ts f s t (rq), a (q) ts = N p=q ∞ k=1 k l=−k A (p) kl ηl−s k+t (Rpq, Opq). (4.30) Here, ηl−s k+t (Rpq, Opq) is the expansion coefﬁcient obtained by consecutive applica- tion of (4.13) and (4.25). In their calculation, one of three options—(4.13), (4.22) or (4.24)—is used depending on the relative position of pth and qth particles. By putting all the parts together, we get T (0) (rq) = ∞ t=1 t s=−t A (q) ts Fs t (rq) + ∞ t=0 t s=−t a (q) ts + c (q) ts f s t (rq). (4.31) Substitution of (4.31) and T (q) in the form (4.7) but written in qth local basis into (2.12) gives an inﬁnite set of linear equations with unknowns A (q) ts , analogous to (4.12) (ωq = λq/λq): 1 (ωq − 1) ωq Qs t (ξq0) Ps t (ξq0) − Q s t (ξq0) P s t (ξq0) A (q) ts + a (q) ts = −c (q) ts . (4.32) 4.5 RUC Likewise (2.33), the above solution can be used for evaluation of the effective conductivity of composite with spheroidal inclusions by combining it with Maxwell’s model. An alternate, advanced tool for this purpose is RUC model: here, we discuss it brieﬂy. For simplicity sake, we assume all the spheroids entering the unit cell oriented in x3-direction: considering the case of arbitrarily oriented spheroids involves some extra algebra but does not meet any other difﬁculties [39]. 4.5.1 Periodic Potentials ToapplytheproceduredescribedinSect.2.5,weﬁrstintroducetheperiodicpotentials analogous to Y∗ ts (2.38): F∗ ts (r, d) = k Fs t (r + ak, d) , (4.33)
- 42. 138 V. I. Kushch where summation is made over all the integer k1, k2 and k3. The solution in the matrix domain is given by the (2.36), (2.37), where now the pth lattice disturbance T ∗(p) dis (rp) = ∞ t=1 t s=−t A (p) ts F∗ ts(rp, dp). (4.34) The solution in the form (2.36), (2.37) satisﬁes the periodicity conditions. In fact, what we need to complete the solution is to ﬁnd local expansion of the functions F∗ ts(rp, dp) in a vicinity of qth inclusion in terms of spheroidal solid harmonics. In the case p = q, we apply the formula (4.13) to all the terms of the sum (4.33) but one with k = 0 to obtain, after change of summation order, F∗ ts(rq, dq) = Fs t rq, dq + ∞ k=0 |l|≤k η∗ tk,s−l 0, dq, dq f l k rq, dq , (4.35) where the expansion coefﬁcients are the triple inﬁnite (lattice) sums η∗s−l tk (R, d1, d2) = k=0 ηs−l kt (R + ak, d1, d2) . (4.36) In the case p = q, rp = Rpq + rq and F∗ ts(rp, dp) = ∞ k=0 |l|≤k ηs−l tk Rpq, dp, dq + η∗ tk,s−l Rpq, dp, dq f l k rq, dq . (4.37) Recall, in RUC model Rpq is taken as a minimal distance between any two particles of pth and qth lattices, so Rpq < Rpq + ak for any k = 0. As was discussed above, the ﬁrst term, ηs−l tk in (4.33) can be evaluated from the appropriate formula. Provided the RUC size a is sufﬁciently large, the formula (4.13) can be used for evaluating the lattice sum η∗s−l tk . Speciﬁcally, η∗ tk,s−l Rpq, dp, dq = k=0 (1) ηs−l tk Rpq + ak, dp, dq (4.38) = atk ∞ r=0 d1 2 2r Mtkr dp, dq Y∗ t+k+2r,s−l Rpq , where Y∗ t+k+2r,s−l Rpq are the standard lattice sums of spherical multipoles (2.40). After we found the local expansions (4.35) and (4.37), the problem is effectively reduced to a set of single inclusion problems. An inﬁnite linear set of equations with unknowns A (q) ts has the form (4.32), where now
- 43. Multipole Expansion Method in Micromechanics of Composites 139 a (q) ts = N p=1 ∞ k=1 k l=−k A (p) kl η∗ tk,s−l Rpq, dp, dq . (4.39) 4.5.2 Effective Conductivity The effective conductivity tensor ∗ of composite is given by (1.1). In view of the temperature ﬁeld periodicity, averaging the temperature gradient in composite with spheroidal inclusions follows the same way as in the spherical case and yields ∇T = G. The macroscopic ﬂux q is given by (1.9) where integration is made now over the spheroidal surfaces Sq : ξq = ξq0. To simplify derivation, we perform it for N = 1 omitting the q index and, then, will write the formula for a general case. For the composite with isotropic matrix we consider, the normal component heat ﬂux qn = q · n at the spheroidal surface equals qn = qξ = −λ∇T · eξ = −λ ξh d ∂T ∂ξ (4.40) In this case, (1.9) simpliﬁes to q λ0 = −G − 1 V S T (0) n − ∂T (0) ∂n r dS. (4.41) The surface integration uses the local expansion (4.31), from where T (0) = ∞ t=1 t s=−t (t − s)! (t + s)! Ats Qs t (ξ) + (ats + cts) Ps t (ξ) χs t , (4.42) ∂T ∂n = ξh d ∞ t=1 t s=−t (t − s)! (t + s)! Ats Q s t (ξ) + (ats + cts) P s t (ξ) χs t . Here, χs t = χs t (η, ϕ); ats are given by (4.39). At the interface S : ξ = const, r = d − 2ξχ−1 1 e1 + ξχ1 1e2 + ξχ0 1e3 , (4.43) n = eξ = h − 2ξχ−1 1 e1 + ξχ1 1e2 + ξχ0 1e3 . By substituting these formulas into (4.41) we get 1 h T (0) n − ∂T (0) ∂n r = 2 ξξ ∂T (0) ∂ξ − ξT (0) χ−1 1 e1 (4.44) + ξT (0) − ξξ ∂T (0) ∂ξ χ1 1e2 + ξ T (0) − ξ ∂T (0) ∂ξ χ0 1e3
- 44. 140 V. I. Kushch Before integrating this expression, we note that f 0 1 (r, d) − ξ ∂ f 0 1 (r, d) ∂ξ ≡ 0; ξ f 1 1 (r, d) − ξξ ∂ f 1 1 (r, d) ∂ξ ≡ 0. (4.45) Also, it is directly testable that ξ ξQ 0 1 − Q0 1 = 1 ξ ; 1 2 ξQ1 1 − ξξQ 1 1 = 1 ξ ; (4.46) and hence F0 1 (r, d) − ξ ∂F0 1 (r, d) ∂ξ = − 1 ξ 2 χ0 1(η, ϕ); (4.47) ξF1 1 (r, d) − ξξ ∂F1 1 (r, d) ∂ξ = 1 ξ χ1 1(η, ϕ). The formula (4.41) readily transforms to q λ0 = −G − 1 V d2 2π 0 1 −1 T (0) n − ∂T (0) ∂n r ξ0 h dηdϕ. By taking Eqs.(4.42)–(4.47) and orthogonality of the surface harmonics χs t into account we ﬁnd readily that 2π 0 1 −1 T (0) − ξ ∂T (0) ∂ξ χ0 1dηdϕ = − 4π 3ξ 2 A10; (4.48) 2π 0 1 −1 ξξ ∂T (0) ∂ξ − ξT (0) χ−1 1 dηdϕ = 4π 3ξ A11; and, ﬁnally, q λ0 = −G + 4πd2 3a3 Re (A10e3 − 2A11e1) . (4.49) In the limiting case where a spheroid degenerates into a sphere, Eq.(4.49) is expected to reduce to (2.47). It is pertinent to mention here that (4.49) can be derived directly from Eq.(2.47)—and this derivation is much easier as compared with that performed above. First, we recognize that the overall structure of Eq.(4.49) is pre-determined by (1.9), so we only need to ﬁnd the dipole moments entering this formula linearly. Next, (4.5) provides the necessary relationship between the
- 45. Multipole Expansion Method in Micromechanics of Composites 141 moments of spherical and spheroidal multipole ﬁelds. For t = 1, the scaling factor equals (−1)sd2/3: as would be expected, by introducing this factor into (2.47) we immediately get (4.49). Noteworthy, the effective conductivity of composite with spheroidal inclusions depends not only on the volume fraction and conductivity of disperse phase but also on the shape, arrangement and orientation of inclusions. Even for simplest cubic symmetry case, this composite is anisotropic at macro level [35]. The inﬁnitely thin oblate spheroid can be used to model penny-shape crack or superconducting platelet. Overall conductivity of solid is greatly affected by presence of these inhomogeneities although their volume content is equal to zero [40]. 4.6 Elasticity Problem 4.6.1 Vectorial Partial Solutions of Lame Equation The following regular vectorial partial solutions f (i) ts have been introduced by [33, 34]: f (1) ts = e1 f s−1 t−1 − e2 f s+1 t−1 + e3 f s t−1; (4.50) f (2) ts = 1 (t + 1) e1(t − s + 1) f s−1 t + (t + s + 1)e2 f s+1 t − e3s f s t ; f(3) ts = e1 − (x1 − ix2)D2 f s−1 t+1 − (ξ2 0 − 1)D1 f s t + (t − s + 1)(t − s + 2)βt f s−1 t+1 + e2 (x1 + ix2)D1 f s+1 t+1 − (ξ2 0 − 1)D2 f s t + (t + s + 1)(t + s + 2)βt f s+1 t+1 + e3 x3D3 f s t+1 − ξ2 0D3 f s t − (t − s + 1)(t + s + 1)βt f s t+1 . In (4.50), ei are the complex Cartesian vectors (2.11) and Di are the differential operators (2.10). The irregular vectorial partial solutions F(i) ts are obtained from (4.50) by replacing the indext with −(t + 1) and f s t with Fs t . In (4.50), f(1) ts and f(2) ts are the vectorial harmonic functions whereas f (3) ts is the vectorial biharmonic function. It contains the harmonic term ξ2 0∇ f s t added in spirit of [70] to simplify the f(3) ts and Tξ(f (3) ts ) expressions at the interface ξ = ξ0. The vectorial harmonics (3.1) do not apply to spheroid; instead we will use the vectorial surface harmonics in the form C ( j) ts (η, ϕ) = ej χ sj t (η, ϕ), where s1 = s − 1, s2 = s + 1 and s3 = s [43]. At the spheroidal surface ξ = ξ0, the functions f(i) ts can be written as f (1) ts = P−s+1 t−1 C (1) t−1,s − P−s−1 t−1 C (2) t−1,s + P−s t−1C (3) t−1,s (4.51) f (2) ts = 1 (t + 1) (t − s + 1)P−s+1 t C (1) ts + (t + s + 1)P−s−1 t C (2) ts − sP−s t C (3) ts ;
- 46. 142 V. I. Kushch f (3) ts = (t − s + 2)ξ0 P−s+1 t + (t − s + 2) − 1 + (t − s + 1)βt P−s+1 t+1 C (1) t+1,s − (t − s)ξ0 P−s−1 t + (t + s + 2) − 1 + (t + s + 1)βt P−s−1 t+1 C (2) t+1,s + (t − s + 1)ξ0 P−s t − Cts P−s t+1 C (3) t+1,s where Ps t = Ps t (ξ0), C ( j) ts = C ( j) ts (η, ϕ) and Cts is deﬁned in (3.31). In compact form, f(i) ts S = 3 j=1 U M ji ts (ξ0, ν) C ( j) t+ j−2,s. (4.52) Analogously, for the irregular solutions we have F (i) ts S = 3 j=1 UG ji ts (ξ0, ν) C ( j) t− j+2,s. (4.53) At the spheroidal surface ξ = const, the traction vector Tn = σ · n can be written as 1 2μ Tξ(u) = ν 1 − 2ν eξ (∇ · u) + ξη d ∂ ∂ξ u + 1 2 eξ × (∇ × u) . (4.54) For the vectorial partial solutions (4.50), this yields 1 2μ Tξ f (i) ts S = 3 j=1 T M ji ts (ξ0, ν) C ( j) t+ j−2,s; (4.55) 1 2μ Tξ F (i) ts S = 3 j=1 T G ji ts (ξ0, ν) C ( j) t− j+2,s. For the explicit expressions of T M ji ts and T G ji ts , see [34, 37]. The net force vector T is non-zero for the functions F(3) 1s only: T F (3) 10 = 16μπd(ν−1)e3; T F (3) 11 = −T F (3) 1,−1 = −32μπd(ν−1)e1 (4.56) Three functions with non-zero net moment M are M F (2) 10 = − 2μπ 3 d2 e3; M F (2) 11 = M F (2) 1,−1 = 4μπ 3 d2 e1. (4.57) Hence, the singular solutions S (3) 1s and S (3) 1s enter the series expansion only if the total force and torque, respectively, is non-zero.
- 47. Multipole Expansion Method in Micromechanics of Composites 143 4.6.2 Single Inclusion Problem The problem statement is analogous to that in Sect.3.2, with Tξ instead of Tr in the interface conditions (3.12). The far load in the form of displacement ﬁeld u f ar and the displacement in the inclusion u(1) are given by the series (3.13) and (3.15), respectively, where the regular solutions u (i) ts (3.6) are replaced with their spher- oidal counterparts, f(i) ts . In the case of linear u f ar = E · r, the non-zero expansion coefﬁcients c (i) ts are c (3) 00 = d 3γ0(ν0) (E11 + E22 + E33), c (1) 20 = d 3 (2E33 − E11 − E22), (4.58) c (1) 21 = −c (1) 2,−1 = d (E13 − i E23) , c (1) 22 = c (1) 2,−2 = d (E11 − E22 − 2i E12) . In the matrix domain, u(0) = u f ar + udis, where the disturbance ﬁeld udis(r) is written as the multipole expansion series udis(r) = i,t,s A (i) ts F (i) ts (r, d). (4.59) We substitute (4.59), together with (3.13) and (3.15), into the ﬁrst of conditions (3.12). By applying (4.52) and (4.53), we get i,t,s c (i) ts 3 j=1 U M ji ts (ξ0, ν0) C ( j) t+ j−2,s (4.60) + i,t,s A (i) ts 3 j=1 UG ji ts (ξ0, ν0) C ( j) t− j+2,s = i,t,s d (i) ts 3 j=1 U M ji ts (ξ0, ν1) C ( j) t+ j−2,s. The orthogonality property of the complex-valued vectors C ( j) ts enables reducing the vectorial functional equality (4.60) to an inﬁnite set of linear algebraic equations. Convenient for the computer algebra form of this system is UGt (ξ0, ν0)At + UMt (ξ0, ν0)ct = UMt (ξ0, ν1)dt (t = 1, 2, . . .); (4.61) where the vector At contains the unknowns A (i) t+i−2,s, the vectors at and dt include a (i) t−i+2,s and d (i) t−i+2,s, respectively. Obtaining the second set of equations from the traction vector continuity condition TGt (ξ0, ν0)At + TMt (ξ0, ν0)ct = TMt (ξ0, ν1)dt . (4.62) follows the same way (for more details, see [34]).
- 48. 144 V. I. Kushch The solution we obtain is complete and valid for any non-uniform far ﬁeld. For the polynomial far ﬁeld of order tmax, this solution is exact and conservative, i.e., is given by the ﬁnite number of terms with t ≤ tmax. This result is consistent with [28]; in particular, tmax = 1 gives us a complete solution of the Eshelby problem. And, to complete this section, we note that the derived solution is also valid in the limiting case of inﬁnitely thin oblate spheroid often used to model the penny-shaped cracks. The normal opening mode stress intensity factor (SIF) KI is deﬁned by KI = lim r→0 √ 2πrσ33 = √ πd lim ξ→1 ξσ33, (4.63) where r is the distance from the point in the plane z = 0 outside the crack to the crack’s tip. An asymptotic analysis of the stress ﬁeld near the crack’s tip gives a series expansion of SIF: d π KI (ϕ) 2μ = ∞ t=0 t s=−t (−1) (t+s) 2 A (1) ts + is (t + 1) A (2) t+1,s (4.64) + 4(1 − ν) t(2t − 1) − (1 − 2ν) A (3) ts exp (isϕ) , where the prime over the internal sum means that it contains only the terms with (t + s) even. For the details of derivation, see [38]. 4.6.3 Re-expansion Formulas for the Lame Solutions Translation. Let r1 = R + r2 Then, F (i) ts (r1) = 3 j=1 ∞ k=0 k l=−k η (i)( j) tksl (R, d1, d2) f ( j) kl (r2, d2) , (4.65) where η(1)(2) tksl = η(1)(3) tksl = η(2)(3) tksl = 0; η(i)(i) tksl = ηs−l t+2−i,k−2+i ; (4.66) η (2)(1) tksl = s t + l k ηs−l t,k−1 η (3)(2) tksl = 2 s t + l k ηs−l t−1,k; η (3)(1) tksl = 2 l k s t + l (k − 1) + Ck−2,l − C−(t+1),s ηs−l t−1,k−1 + (2k − 1) × ∞ m=0 (−1)m X3 d2 ηs−l t−1,k+2m − d1(ξ10)2 ηs−l t,k+2m + d1(ξ20)2 ηs−l t−1,k+2m+1 .
- 49. Multipole Expansion Method in Micromechanics of Composites 145 In (4.66) ηs−l tk are the expansion coefﬁcients for the scalar spheroidal harmonics Fs t (4.13). These, as well as the other (R2R and S2S) expansions have been derived by [33]. Rotation. The re-expansion formulas for the partial irregular solutions F (i) ts due to rotation of coordinate frame r1 = O12 · r2 are: F (i) ts (r1, d1) = 3 j=1 t+i− j k=0 k l=−k R (i)( j) tksl (w12, d1, d2) F ( j) kl (r2, d2) , (4.67) where R (i)( j) tksl = i α= j t+i−α p=k+ j−α K(1)(i)(α) t, p+α−i, s (d1) K (2)(α)( j) p, k+ j−α,l (d2) S p−s,p−l 2p (w12) (4.68) + δi3δj1(2k − 1) t n=k (ξ10)2 R (3)(3) tnsl − (ξ20)2 R (2)(2) tnsl and K (β)(i)( j) tks = 0 for i < j; K (β)(i)(i) tks = K (β) t−i+2,k−i+2; (4.69) K (β)(2)(1) tks = s k − s t K (β) tk , K (β)(3)(2) tks = 4(1 − ν) s k − s t K (β) t−1,k−1; K (β)(3)(1) tks = C−(k+1),s − C−(t+1),s K (β) t−1,k−1 − s (k − 1) K (β)(3)(2) tks . Here, K (β) tk are given by the formulas (4.6), β = 1, 2. In (4.67), we keep in mind that the vectorial functions standing in the opposite sides of equality are written in their local coordinates and components. These formulas are written for the most general case d1 = d2 and ξ10 = ξ20. The analogous formulas for the regular solutions are exact and ﬁnite: for their explicit form, see [34, 39]. 4.6.4 FCM and RUC Now, we have in hands all the necessary theory to solve the elasticity problems for multiple spheroidal inclusions. We take the displacement ﬁeld in the matrix domain in the form (3.32), where now multipole expansion of the disturbance caused by p-th inclusion is written as u (p) dis(rp) = i,t,s A (i)(p) ts F (i) ts (rp, dp). (4.70)
- 50. 146 V. I. Kushch Fulﬁlling the interface conditions gives us the linear set of equations similar to (4.61), (4.62) UGt (ξq0, ν0)A (q) t + UMt (ξq0, ν0) a (q) t + c (q) t = UMt (ξq0, νq)d (q) t ; (4.71) TGt (ξq0, ν0)A (q) t + TMt (ξq0, ν0) a (q) t + c (q) t = TMt (ξq0, νq)d (q) t . Here, ct is given by (4.58) and a (q) t is the contribution of all other inclusions (with p = q) to the ﬁeld around the qth inclusion: a (q) t = p=q ∞ k=1 η (p)(q) kt A (p) k , (4.72) in scalar form, a (i)(q) ts = N p=q 3 j=1 ∞ k=0 k l=−k A ( j)(p) kl η ( j)(i) klts Rpq, dp, dq . (4.73) Here, we assumed all the spheroids equally oriented: Opq = I. The case of arbitrarily oriented spheroids is considered elsewhere [39]. By analogy with (3.39)–(3.41), one can use this model to evaluate the effective stiffness of composite in spirit of Maxwell’s method. Extension of this solution to the periodic, RUC type model is analogous to that for the spherical inclusions and so we do not repeat it here. In fact, it mostly consists in replacing the expansion coefﬁcients (4.66) with their periodic counterparts in the matrix of linear system (4.71). 4.6.5 Effective Stiffness Tensor The effective stiffness tensor C∗ of composite is given by (1.10). In view of the displacement ﬁeld periodicity, averaging the strain in composite with spheroidal inclusions follows the same way as in the spherical case and yields ε = E. The macroscopic stress σ is given by Eq.(1.13) where integration is made now over the spheroidal surfaces Sq : ξq = ξq0. The integration procedure closely resembles that exposed in Sect.3 and is straightforward although somewhat laborious. An alternate approach to obtaining the expressions for effective properties was discussed already in this Section, in the conductivity context. This approach extends to the elasticity problem: namely, an expression for the macroscopic stress in spher- ical particle composite (3.51) transforms to the analogous formula for the aligned spheroidal particle composite by taking into account that for d → 0 V(1) 00 (r, d) ≈ N0U(1) 00 (r); V(3) 2,s(r, d) ≈ NsU(3) 2,s(r);
- 51. Multipole Expansion Method in Micromechanics of Composites 147 where the scaling factor Ns = (−1)sd2/3. By inserting this factor into (3.51) we obtain immediately the desired formulas: σ11 + σ22 + σ33 3k0 = (E11 + E22 + E33) + 1 + 4μ0 3k0 N q=1 dp A (1)(q) 00 ; (4.74) 2 σ33 − σ11 − σ22 2μ0 = (2E33 − E11 − E22) − 4 (1 − ν0) N q=1 dp A (3)(q) 20 ; σ11 − σ22 − 2i σ12 2μ0 = (E11 − E22 − 2iE12) − 8 (1 − ν0) N q=1 dp A (3)(q) 22 ; σ13 − i σ23 2μ0 = (E13 − iE23) + 2 (1 − ν0) N q=1 dp A (3)(q) 21 . where dp = 4π dp 2 /3a2 and k = 2μ(1+ν) 3(1−2ν) . 5 Spherical Particles Reinforced Composite with Transversely-Isotropic Phases In the Cartesian coordinate system Ox1x2x3 with Ox3 axis being the anisotropy axis of transversely isotropic material, an explicit form of the generalized Hooke’s law is ⎛ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝ σ11 σ22 σ33 σ23 σ13 σ12 ⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠ = ⎛ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝ C11 C12 C13 0 0 0 C12 C11 C13 0 0 0 C13 C13 C33 0 0 0 0 0 0 2C44 0 0 0 0 0 0 2C44 0 0 0 0 0 0 (C11 − C12) ⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠ ⎛ ⎜ ⎜ ⎜ ⎜ ⎜ ⎜ ⎝ ε11 ε22 ε33 ε23 ε13 ε12 ⎞ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠ . (5.1) Here, two-indices notation Ci j is adopted. The components of stress tensor σ satisfy the equilibrium equations ∇ · σ = 0 and the small elastic strain tensor ε is related to the displacement vector u by ε = 1 2 ∇u + (∇u)T . 5.1 Background Theory Based on representation of general solution in terms of three potential functions [70], Kushch [43] has introduced the following, full for ν1 = ν2 set of regular vectorial solutions v ( j) ts :
- 52. 148 V. I. Kushch v ( j) ts (r) = f s−1 t (rj , dj )e1 − f s+1 t (rj , dj )e2 + kj √ νj f s t (rj , dj )e3 ( j = 1, 2); (5.2) v (3) ts (r) = f s−1 t (r3, d3)e1 + f s+1 t (r3, d3)e2; t = 0, 1, 2, . . . ; |s| ≤ t + 1. In (5.2), ν3 = 2C44/ (C11 − C12) whereas ν1 and ν2 are the roots of equation C11C44ν2 − (C44)2 − C11C33 − (C13 + C44)2 ν + C33C44 = 0. (5.3) Expressions of k1 and k2 are kj = C11νj − C44 C13 + C44 = νj (C13 + C44) C33 − νj C44 , j = 1, 2 . (5.4) The modiﬁed Cartesian rj and prolate spheroidal coordinates ξj , ηj , ϕj are given for νj < 1 by x1 + ix2 = x1 j + ix2 j = dj ¯ξj ¯ηj exp(iϕj ), x3 = √ νj x3 j = √ νj dj ξj ηj ; (5.5) In the case νj > 1, the oblate spheroidal coordinates must be used. The system (5.5) is chosen in a way that ξj = ξj0 = const at the spherical surface r = R; i.e., S is the ξ-coordinate surface of (5.5). We provide this by deﬁning dj = R/ξj0, ξj0 = νj / νj − 1 . (5.6) In this case, moreover, we have ηj = θ and ϕj = ϕ for r = R, where (r, θ, ϕ) are the ordinary spherical coordinates corresponding to the Cartesian ones (x1, x2, x3). This is the key point: no matter how complicated solution in the bulk is, at the interface we get the linear combination of regular spherical harmonics Ys t (θ, ϕ). Under this circumstance, fulﬁlling the contact conditions at interface is straightforward. The explicit form of the irregular vectorial solutions V ( j) ts is given by the Eq.(5.2), with the replace f s t by Fs t . According to [23], Fs t = f s t ≡ 0 for |s| > t. This condition makes it impossible to represent some irregular solutions in the form (5.2). To resolve this issue, Kushch [43] has introduced the following, additional to (4.4) functions of the form Ft+k t (r, d) = 1 (2t + k)! Qt+k t (ξ) Pt+k t (η) exp [i (t + k) ϕ] , (5.7)
- 53. Multipole Expansion Method in Micromechanics of Composites 149 (k = 0, 1, 2, . . .) where Pt+k t (p) = (2t + k)! (1 − p2)(t+k)/2 1 p 1 p · · · 1 p t+k Pt (p) (dp)t+k = (2t + k)! (1 − p2)(t+k)/2 It+k (5.8) for 0 ≤ p ≤ 1; for p < 0, Pt+k t (p) = (−1)k Pt+k t (−p). It is straightforward to show that the functions (5.7) are the irregular solutions of Laplace equation. In contrast to (4.4), they are discontinuous at x3 = 0. In the general series solution, however, these breaks cancel each other and give the continuous and differentiable expressions of the displacement and stress ﬁelds. Remarkably, the functions Ft+k t are introduced in a way that for them are valid all the principal results including the re-expansion formulas (4.13) and (4.15). At the spherical surface r = R, the functions V (i) ts and v (i) ts can be written in the compact form as V(i) ts S = 3 j=1 UG ji ts C ( j) ts , v(i) ts S = 3 j=1 U M ji ts C ( j) ts , (5.9) where C ( j) ts (θ, ϕ) is deﬁned in (4.51). In (5.9), the matrix UGts = UG i j ts = ⎛ ⎜ ⎜ ⎝ Qs−1 t (ξ10) Qs−1 t (ξ20) Qs−1 t (ξ30) −Qs+1 t (ξ10) −Qs+1 t (ξ20) Qs+1 t (ξ30) k1√ ν1 Qs t (ξ10) k2√ ν2 Qs t (ξ20) 0 ⎞ ⎟ ⎟ ⎠ ; (5.10) UMts has the form (5.10), where Qs t are replaced with Ps t . To satisfy the stress boundary conditions, we need the similar representation for the traction vector Tn = σ · n. For the explicit expressions of Tn(v ( j) ts ) at the surface S, see [43]. These and analogous expressions for Tn(V ( j) ts ) also can be written in the compact form Tn(V ( j) ts ) S = 3 j=1 T G ji ts C ( j) ts , Tn(v ( j) ts ) S = 3 j=1 T M ji ts C ( j) ts . (5.11) For the deﬁniteness sake, we assume here and below ν1 = ν2. In the case of equal roots ν1 = ν2, solution (5.2) is not general because of f (1) ts ≡ f (2) ts . In this case, to get a complete set of independent solutions, v (2) ts can be taken in the form [43]
- 54. 150 V. I. Kushch v (2) ts (r) = d1 x3∇ − C13 + 3C44 C13 + C44 i3 f s t (r1, d1) + √ ν1d1 (ξ10)2 ∇ f s t−1(r1, d1). (5.12) For the expression of the corresponding traction vector, see [70]. 5.2 Series Solution Let us consider an inﬁnite solid with a single spherical inclusion of radius R embedded. The matrix and inclusion are made from transversely isotropic materials and perfectly bonded: u+ − u− S = 0; Tn u+ − Tn u− S = 0. (5.13) InthisSection,alltheparametersassociatedwiththematrixandinclusionaredenoted by the superscript “−” and “+”, respectively. We assume the anisotropy axes of both the matrix and inclusion materials to be arbitrarily oriented and introduce the material-related Cartesian coordinate systems Ox− 1 x− 2 x− 3 and Ox+ 1 x+ 2 x+ 3 with common origin in the center of inclusion. The point coordinates and the vector components in these coordinate systems are related by x+ i = Oi j x− j , u+ i = Oi j u− j (5.14) where O is the rotation matrix. Transformation of the vectors ii uses the formula i+ i = Ω∗ i j i− j , where O∗ = D−1 OD and D = ⎛ ⎝ 1 1 0 −i i 0 0 0 1 ⎞ ⎠ . (5.15) The displacement ﬁeld within the inclusion u+ can be expanded into a series over the regular solutions v ( j) ts (5.2): u+ = j,t,s d ( j) ts v ( j) ts r+ , ⎛ ⎝ j,t,s = 3 j=1 ∞ t=0 |s|≤t+1 ⎞ ⎠ (5.16) whered ( j) ts aretheexpansioncoefﬁcientstobedeterminedfromthecontactconditions (5.13). The displacement vector in the matrix domain is a sum of far ﬁeld u f ar = E · r− and disturbance udis whose multipole type expansion in terms of V ( j) ts is given by u− = u f ar + udis = E · r− + j,t,s A ( j) ts V ( j) ts r− . (5.17)

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment